- Home
- Documents
- Amber Mace - DiVA 782425/ molecular dynamics approach Amber Mace, ... from the quantum scale to the macroscopic Amber Mace, ... Qingling Liu, Amber Mace and Niklas Hedin, Applied ...

Published on

19-Mar-2018View

212Download

0

Transcript

Multiscale Modeling of Molecular Sieving in LTA-type Zeolites Fromthe Quantum Level to the MacroscopicAmber Macemailto:amber.mace@mmk.su.seMultiscale Modeling of MolecularSieving in LTA-type ZeolitesFrom the Quantum Level to the MacroscopicAmber Macemailto:amber.mace@mmk.su.seDoctoral Thesis in Physical Chemistry 2015Department of Materials and Environmental ChemistryStockholm UniversitySE-10691 Stockholm, SwedenFaculty Opponent:Prof. Tina Dren, Department of Chemical Engineering, University of Bath,UKEvaluation committee:Prof. Natalia Skorodumova, School of Industrial Engineering and Manage-ment, KTH Royal Institute of Technology, SwedenProf. Kersti Hermansson, Department of Chemistry, Uppsala UniversityProf. Michael Odelius, Department of Physics, Stockholm University, SwedenSubstitute:Prof. Olle Edholm, Department of Theoretical Physics, KTH Royal Instituteof Technology, SwedenChairman and coordinator:Prof. Arnold Maliniak, Department of Materials and Environmental Chem-istry, Stockholm University, SwedencAmber Mace, Stockholm 2015ISBN 978-91-7649-081-5Printed in Sweden by USAB, Stockholm 2015Distributor: Department of Materials and Environmental Chemistry, Stockholm UniversityThis thesis is dedicated to Annabelle and her sister.AbstractLTA-type zeolites with narrow window apertures coinciding with the approxi-mate size of small gaseous molecules such as CO2 and N2 are interesting candi-dates for adsorbents with swing adsorption technologies due to their molecularsieving capabilities and otherwise attractive properties. These sieving capabili-ties are dependent on the energy barriers of diffusion between the zeolite pores,which can be fine-tuned by altering the framework composition. An ab initiolevel of theory is necessary to accurately describe specific gas-zeolite interac-tion and diffusion properties, while it is desirable to predict the macroscopicscale diffusion for industrial applications. Hence, a multiscale modeling ap-proach is necessary to describe the molecular sieving phenomena exhaustively.In this thesis, we use several different modeling methods on different lengthand time scales to describe the diffusion driven uptake and separation of CO2and N2 in Zeolite NaKA. A combination of classical force field based mod-eling methods are used to show the importance of taking into account boththermodynamic, as well as, kinetic effects when modeling gas uptake in nar-row pore zeolites where the gas diffusion is to some extent hindered. For amore detailed investigation of the gas molecules pore-to-pore dynamics inthe material, we present a procedure to compute the free energy barriers ofdiffusion using spatially constrained ab initio Molecular Dynamics. With thisprocedure, we seek to identify diffusion rate determining local properties of theZeolite NaKA pores, including the Na+-to-K+ exchange at different ion sitesand the presence of additional CO2 molecules in the pores. This energy barrierinformation is then used as input for the Kinetic Monte Carlo method, allow-ing us to simulate and compare these and other effects on the diffusion drivenuptake using a realistic powder particle model on macroscopic timescales.List of PapersThe following papers I-IV, referred to in the text by their Roman numerals, areincluded in this thesis.PAPER I NaKA sorbents with high CO2-over-N2 selectivity and high ca-pacity to adsorb CO2Qingling Liu, Amber Mace, Zoltan Bacsik, Junliang Sun, Aatto Laak-sonen and Niklas Hedin, Chem. Comm. 2010, 46, 45024504DOI: 10.1039/C000900HSpecific contributions: planned and performed the modeling, contributedto the writingPAPER II Role of Ion Mobility in Molecular Sieving of CO2 over N2 withZeolite NaKAAmber Mace, Niklas Hedin and Aatto Laaksonen, J. Phys. Chem. C2013, 117, 2425924267DOI: 10.1021/jp4048133Specific contributions: lead role in this project, planned and performedall modeling, lead role in writingPAPER III Free energy barriers for CO2 and N2 in zeolite NaKA: an abinitio molecular dynamics approachAmber Mace, Kari Laasonen and Aatto Laaksonen, Phys. Chem. Chem.Phys. 2014, 16,166172.DOI: 10.1039/c3cp52821aSpecific contributions: lead role in this project, performed all modeling,lead role in writingPAPER IV Temporal coarse graining of CO2 diffusion in Zeolite NaKA;from the quantum scale to the macroscopicAmber Mace, Mikael Leetmaa and Aatto Laaksonen, To be submitted.Specific contributions: lead role in this project, planned and performedall modeling, lead role in writingReprints were made with permission from the publishers.http://dx.doi.org/10.1039/C000900Hhttp://dx.doi.org/10.1021/jp4048133http://dx.doi.org/10.1039/c3cp52821aAdditional papers by the author, which are not included in the thesis.PAPER V Oxygen-oxygen correlations in liquid water: Addressing thediscrepancy between diffraction and extended x-ray absorption fine-structure using a novel multiple-data set fitting techniqueKjartan Thor Wikfeldt, Mikael Leetmaa, Amber Mace, Anders Nilssonand Lars G. M. Pettersson, J. Chem. Phys. 2010, 132,104513104522DOI: 10.1063/1.3330752PAPER VI Oxide clusters as source of the third oxygen atom for the for-mation of carbonates in alkaline earth dehydrated zeolitesAlexander Larin, Andrey Rybakov, Georgii M. Zhidomirov, Amber Mace,Aatto Laaksonen and Daniel Vercauteren, J. Catal. 2011, 281, 212221DOI: 10.1016/j.jcat.2011.05.002PAPER VII Carbonate "door" in the NaKA zeolite as the reason of higherCO2 uptake relative to N2Alexander Larin, Amber Mace, Andrey Rybakov and Aatto Laaksonen,Microporous Mesoporous Mater. 2012, 162, 98104DOI: 10.1016/j.micromeso.2012.06.005PAPER VIII Adsorption kinetics for CO2 on highly selective zeolites NaKAand nano-NaKAOcean Cheung, Zoltan Bacsik, Qingling Liu, Amber Mace and NiklasHedin, Applied Energy 2013, 112, 13261336.DOI: 10.1016/j.apenergy.2013.01.017PAPER IX Crystal structure and magnetic properties of the S=1/2 quan-tum spin system Cu7(TeO3)6F2 with mixed dimensionalityShichao Hu, Amber Mace, Mats Johnsson, Vladimir Gnezdilov, PeterLemmens, Joshua Tapp and Angela Mller, Inorg. Chem. 2014, 53,76617667.DOI: 10.1021/ic5009686PAPER X K+ Exchanged Zeolite ZK-4 as a Highly Selective Sorbent forCO2Ocean Cheung, Zoltan Bacsik, Panagiotis Krokidas, Amber Mace, AattoLaaksonen, Niklas Hedin, Langmuir 2014, 30, 96829690.DOI: 10.1021/la502897phttp://dx.doi.org/10.1063/1.3330752http://dx.doi.org/10.1016/j.jcat.2011.05.002http://dx.doi.org/10.1016/j.micromeso.2012.06.005http://dx.doi.org/10.1016/j.apenergy.2013.01.017http://dx.doi.org/10.1021/ic5009686http://dx.doi.org/10.1021/la502897pPAPER XI Gas and organic vapour adsorption properties of NOTT-400and NOTT-401: selectivity derived from directed supramolecularinteractionsIlich Ibarra, Amber Mace, Sihai Yang, Junlian Sun, Sukyung Lee, Jong-San Chang, Aatto Laaksonen, Martin Schrder, Xiadong Zou, To be sub-mitted.PAPER XII Nanocellulose-Zeolite Composite Films for Odor EliminationNeda Keshavarzi, Farshid Mashayekhy Rad, Amber Mace, Mohd F.Ansari, Farid Akhtar, Ulrika Nilsson, Lars Berglund, Lennart Bergstrm,To be submitted.Abbreviationsm micrometer (106m)a.u. atomic unitsAIMD ab initio Molecular DynamicsAlPO Aluminum phosphateCHA ChabaziteDFT Density Functional TheoryFAU Faujasitefs femtosecond (1015s)GCMC Grand Canonical Monte CarloGPW Gaussian and plane wavesGTH Goedecker-Teter-HutterKMC Kinetic Monte CarloLTA Linde Type AMD Molecular DynamicsMM Molecular MechanicsMMC Metropolis Monte CarloMOR Mordenitenm nanometer (109m)ns nanosecond (109s)PBC periodic boundary conditionsPBE Perdew-Burke-Ernzerhofps picosecond (1012s)PSA pressure swing adsorptionQC Quantum ChemistrySAPO Silica aluminum phosphateTSA temperature swing adsorptionXRD X-ray diffraction ngstrm (1010m)ContentsAbstract viList of Papers viiAbbreviations xi1 Introduction 151.1 Background . . . . . . . . . . . . . . . . . . . . . . . . . . . 151.2 Zeolites as molecular sieves . . . . . . . . . . . . . . . . . . 161.3 Molecular multiscale modeling . . . . . . . . . . . . . . . . . 182 Diffusionally enhanced CO2-over-N2 selectivity in Zeolite NaKA 232.1 Zeolite A . . . . . . . . . . . . . . . . . . . . . . . . . . . . 232.2 Kinetic molecular sieving . . . . . . . . . . . . . . . . . . . . 252.3 Fine-tuning the effective pore window in Zeolite NaKA . . . . 263 Predicting the CO2 uptake using force field based modeling 293.1 Force fields . . . . . . . . . . . . . . . . . . . . . . . . . . . 293.2 Modeling the thermodynamic effect with Grand Canonical MonteCarlo . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 313.3 Modeling the kinetic effect with Molecular Dynamics . . . . . 333.4 Predicting the total uptake in narrow pore zeolites . . . . . . . 354 Predicting the free energy barriers of diffusion using constrainedAIMD modeling 374.1 Density Functional Theory . . . . . . . . . . . . . . . . . . . 374.2 Periodic DFT-simulations with CP2K . . . . . . . . . . . . . 394.3 Constrained AIMD . . . . . . . . . . . . . . . . . . . . . . . 404.4 Determining the free energy barriers of diffusion in ZeoliteNaKA . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 404.5 Identifying the local diffusion rate-determining properties . . . 425 Scaling up: Coarse graining the time evolution with Kinetic MonteCarlo 495.1 Kinetic Monte Carlo . . . . . . . . . . . . . . . . . . . . . . 495.2 Determining the rate constants . . . . . . . . . . . . . . . . . 535.3 KMC-simulations with KMCLib . . . . . . . . . . . . . . . . 545.4 Modeling the CO2 and N2 uptake in a realistic Zeolite NaKApowder particle model . . . . . . . . . . . . . . . . . . . . . 545.5 Testing the effects of rate-determining properties . . . . . . . 575.6 Adsorption kinetics . . . . . . . . . . . . . . . . . . . . . . . 606 Conclusions and Outlook 63Sammanfattning p svenska lxviiAcknowledgements lxixReferences lxxi1. Introduction1.1 BackgroundAccording to the overwhelming majority of the leading climate research weare in a time where the threat of global warming is immediate [1]. There isstrong scientific support that this is a direct consequence of the vast increaseof emission of greenhouse gases into the atmosphere resulting from the drasticincrease of industrial discharge mainly from burning fossil fuels such as oil,coal, pete and natural gases during the last century [2].In the last few decades development of climate neutral industrial tech-niques have accelerated and the future in this field looks bright giving hopethat the dependence of fossil fuels, given time, can be broken. However, inorder to stop the negative development of the climate we cannot afford to waitand the CO2 discharge into the atmosphere must immediately decrease, drasti-cally. Therefore, developing efficient techniques for capturing CO2 is a neces-sity. Further, these techniques need to be inexpensive to also be afforded bydeveloping countries where the burning of coal is the main energy supply. [3]Typically, flue gas discharge from a coal-fired power plant is composed of81% N2, 5% O2, and 14% CO2 in addition to trace contaminants such as sulfurand nitrogen oxides [4]. However, when studying the separation of CO2 fromthe flue gas bulk, it is necessary to study the unique physical relation betweenCO2 and each other flue gas component separately. In this thesis, the focus hasbeen on the process of separating CO2-from-N2, efficiently and inexpensively,as this has shown to be a challenge due to the similarities of the two molecules.Today, there are several techniques being investigated for this purpose. Themain method currently in use in industries for the separation of CO2 from N2is adsorption with an amine water solution, so-called amine scrubbing. Thisseparation method relies on the difference in the chemical reactivities betweenCO2 and N2, where CO2 has a higher affinity to create chemical bonds, so-called chemisorption, to the amines in the solution [3; 5]. However, breakingthe chemical bonds for regeneration of the liquid substrate to enable a newseparation cycle is commonly executed by boiling the solution. Following thehigh heat capacity of water the cost of amine scrubbing is high, too high to beused extensively, hence, the development of separation substrates needs to be15driven forward.Compared to chemisorption, physical van der Waals or electrostatic inter-actions, referred to as physisorption have lower heats of adsorption. Therefore,it is of great interest to investigate materials, which attract large amounts ofCO2 through weaker non-bonding interactions in order to lower the cost andefficiency of carbon capture and separation techniques and therein increase theuse of these methods.For the separation process, pressure or temperature swing adsorption tech-niques (PSA/TSA) are commonly used. These techniques are based on therelation between the gas pressure or temperature and the chemical potentialbetween the adsorbate and adsorbent [6]. For a gas molecule adsorbed toa material at room temperature and ambient pressure, desorption will occurwhen the temperature is increased enough to provide the system with suffi-cient energy to break the bonds, alternatively, the pressure is decreased to avalue where the chemical potential reaches zero. Increasing the temperatureand decreasing the pressure involve energy costs, which depend on the extentof these, so-called, swings. In turn, the extent of the swings depend on theinteraction energy, or heats of adsorption of the adsorbate to the adsorbent.Therefore, for cost efficient swing cycles it is attractive that this heat of ad-sorption is as low as possible, while still achieving the capacity and selectivityrequired for the uptake and separation process.The minimum electric load imposed on a power plant during such a PSA/TSAprocess was coined as the "parasitic energy" by Lin et al. [7] who also pre-dicted that an intermediate value of the heat of adsorption yields the lowestparasitic energy. This thesis work relates to the possibility that the parasiticenergy could be further decreased by employing kinetic aspects to the CO2-over-N2 separation process, vide infra.1.2 Zeolites as molecular sievesWhen it comes to research on potential adsorbents, porous material, such aszeolites, have received a lot of attention. Zeolites are microporous crystallinealuminum silicates, which both occur naturally and can be synthesized in thelaboratory. Due to their porosity these materials obtain a high surface areagiving them a high capacity for gas adsorption. Also, the pore sizes of thesematerials are in the molecular size range allowing them to function as molecu-lar sieves, distinguishing amongst molecules of different sizes.There is a large variety of zeolites with varying Al-to-Si ratios. The frame-work obtains a negative charge from the Al-atoms, which are in turn neutral-ized by mono or divalent extra-framework cations, generally Na+, K+ or Ca2+16Figure 1.1: Four examples of common Zeolite framework structures: FAU (topleft), CHA (top right), MOR (bottom left) and LTA (bottom right).ions. Zeolites also vary in pore sizes and shapes (four examples are shown inFigure 1.1) where there are two main types:1. Channel-type where the framework is built up by a one or two dimen-sional channel system2. Cage-type where the framework is three dimensional and consists ofcage-like sections of different sizesWhen it comes to separating CO2 from N2 there are two major differencesbetween these two gas molecules which can be exploited in the separation pro-cess: first, CO2 has a quadrupole moment (14 1040 Cm2) almost threetimes as high as that for N2 (4.71040 Cm2) [8]. This provides CO2 witha higher affinity to the zeolite arising from the variations in the electrostaticlandscape of the zeolitic surface. These contributions to the uptake and sep-17aration will in the thesis be referred to as thermodynamic effects. It is thesethermodynamic effects that most gas separation processes, in fact, rely on.Second, CO2 has a slightly smaller kinetic diameter than N2, 3.3 and 3.6 ,respectively [9]. The smaller kinetic diameter of the CO2 molecule entails thatit can squeeze through slightly smaller zeolite pore openings compared the N2molecule. This may seem somewhat counterintuitive to many, however, thekinetic diameter is not a pure size effect neither is it particularly straight for-ward to explain. As a measure, the kinetic diameter, was in fact determinedfor certain gas molecules by, namely, zeolite uptake experiments. Here, thekinetic diameters where determined by identifying the cutoff pore diameterof the zeolite where the particular gas molecule could no longer enter. Thisleads us to believe that the kinetic diameter is more than a pure size measureand that, perhaps, properties of the gas molecule, such as polarizability mayhave "steering" effects. This thesis work has given some clarification to theseideas and will be discussed more in chapter 4. This size selective separationbetween CO2 and N2 will be referred to as the kinetic effect. It is also thissecond, kinetic effect, which this thesis will particularly investigate. Can theseparation be enhanced through size selective molecular sieving and what arethe properties, of the adsorbate as well as the adsorbent, which dictate the rateof diffusion through the porous material?As mentioned, there is a large variety of zeolites. Additionally, there areconsiderable possibilities to alter or synthesize a specific zeolite in order tooptimize its functionality for a certain application. As the focus of the workpresented in this thesis has been on enhancing the CO2-over-N2 selectivitythrough kinetic effects, this investigation has been restricted to narrow porezeolites of LTA-type and how the effective pore window diameter, diffusionrates and, in turn, the CO2-over-N2 selectivity can be altered through cationexchange.1.3 Molecular multiscale modelingIn the last few decades molecular modeling has attained an increasingly im-portant role in molecular research. The exponentially increasing supply ofcomputational resources [10] along with the maturation of modeling methodshave brought molecular modeling and computational chemistry to become anaturally integrated part of the analysis of experimental data, allowing us topredict unknown properties of materials while providing insight to what is go-ing on at the molecular scale. Modeling also opens up for the possibility topredict new materials yet to be synthesized acquiring properties of interest fora specific application.It is not either uncommon that reviewers of higher impact journals ask for18modeling work to support and describe experimental data. Today, just overone year ago, Martin Karplus, Micheal Levitt and Arieh Warshel received theNobel Prize in Chemistry 2013 for their work on the development of multi-scale models for complex chemical systems [11]. This was the well-deservedcertificate showing the important role molecular modeling and computationalchemistry play in molecular research. Just during this last year, I have myselfexperienced a drastic increase in collaboration interests and interest in molec-ular modeling from colleagues working with experiments. I see this increasedinterest with very positive eyes and I am a strong believer that an increasedcollaboration between theoreticians and experimentalists can only improve theresearch of each parts as well as strengthen molecular research as a whole.So what is molecular modeling and, in particular, what is molecular mul-tiscale modeling? Well, molecular modeling is more or less anything from asimple drawing or ball and stick model to advanced computational methods,which act to simulate the behavior of a molecular system. Most or all molec-ular modeling methods are developed from knowledge of the laws of physics,either classical or quantum mechanical. Following this, there are two main cat-egories of computational molecular modeling techniques. Classical molecularmechanics based methods (MM) and quantum chemistry methods (QC).Molecular mechanics is based on classical and statistical mechanics wherethe atoms are treated explicitly and the interatomic interaction in the systemare described by predetermined force fields, which are parametrized eitherto experimental results or quantum chemical calculations. MM methods canfurther be divided in to two main types: Metropolis Monte Carlo Methods(MMC) [12] and Molecular Dynamics methods (MD) [13; 14]. MMC meth-ods randomly sample the systems potential energy surface according to theBoltzmann distribution in search for the minimal energy configuration accord-ing to the defined system ensemble. However, as MMC is a purely statisticalmethod it does not show the molecular systems propagation over time and wecannot get any information on the dynamics of the system. This is, instead,exactly what MD methods model. Here the atomic positions are propagatedin time by solving the Newtonian equation of motion. This results in a deter-ministic trajectory of the atomic movements as a function of time. With theseMM methods relatively large systems and time scales (i.e. m and ns) cangenerally be modeled and the behavior of macroscopic quantities in a systemsuch as pressure, volume and temperate can be determined. The MM methodsused in this thesis will be described more in detail in chapter 3.Quantum chemistry on the other hand is based on the laws of quantummechanics and considers the behavior of the electrons explicitly. This allowsus to investigate the nature of the chemical bonds and interactions in detail.These computations are said to be ab initio from the beginning. Due to19the high computational cost, QC computations are generally limited to smallersystems or specific locations of interest in a material such as a bonding site.Additionally, QC computations can be implemented into both MMC and MDmethods where interatomic interactions energies at each simulation step aredetermined by QC instead of the by the predetermined force fields. Ab initioMolecular Dynamics (AIMD) will be described more in detail in chapter 4.Unfortunately, there is no single modeling method, which is ideal for allapplications and generally the higher accuracy you acquire in your model themore computational time is required, restricting the computations to smallersystems. Therefore, it is critical that the level of theory is adapted to the lengthand timescale of the system to be modeled. The tradeoff between accuracy andsize needs to be adjusted to answer the question at interest with a reasonableaccuracy.Figure 1.2: Multiscale modelingVery often, in order to provide a description of a phenomenon or process ina system exhaustively, it is necessary to extend the modeling work over severallength and time scales (Figure 1.2) and it is this, which is referred to as multi-scale modeling. Multiscale modeling methods often involve transferring infor-mation retrieved from simulation methods with high accuracy but small lengthand time scales to simulation methods treating larger scales, hence, bridgingthe scales together. In particular, when it comes to materials, it is highly at-20tractive to be able to provide macroscopic scale models in order to predict"real" behavior in materials. As neither QC nor MM modeling methods areable to reach macroscopic length and timescales, it is necessary to go beyondatomistic scale modeling methods and employ so-called coarse graining meth-ods. The coarse graining may take place in the spatial dimension where, forexample, several atoms may be bunched together in molecular segments andgiven unitary interaction properties. These interaction properties are, in turn,retrieved from smaller scale (electronic or atomistic) simulations. One exam-ple of a very common use of coarse graining units is for hydrocarbon com-plexes in force field based molecular modeling methods. Here, the hydrogenatoms are not treated explicitly but instead effectively as a united atom com-plex where each specific hydrocarbon segment (-CH, -CH2, -CH3 a.s.o.) isassigned force field parameters mimicking a single atom [15]. However, withspatial coarse-graining even whole functional groups and other larger entitiesof atoms may be treated as a single interaction site. In a similar manner, thetemporal scale can be coarse grained. Temporal coarse graining methods aretoday not as widely used as spatial coarse graining methods but those, whichhave gained more extensive use are based on the Arrhenius rate law [16], ingeneral Kinetic Monte Carlo (KMC) methods [17; 18]. These methods areappropriate for rare event dynamics where the specific rate determining prop-erties for the process of interest can be identified and measured independentlyof other events. Here, it is only the time related to the full process, which isof interest. Therefore, the short time intervals related to each intermediate stepare coarse grained into only one, much longer time step corresponding to thefull process or event. This method will be discussed more in detail in chapter5.This thesis treats an extensive range of length and timescales, from theelectronic scale to the macroscopic scale using a variety of modeling methodswhen investigating the cation exchanged LTA type zeolites and their function-ality as molecular sieves for the separation of CO2 and N2 gases. I startedoff my thesis work on this subject on the atomistic scale using classical forcefield based modeling. Here, MMC and MD were combined in an approachto take into account both the thermodynamic and kinetic effects of the selec-tive uptake of CO2. Next, going down in the multiscale modeling length andtime scale presented in Figure 1.2, I used AIMD to describe the kinetic effectin greater detail. Finally, based on the information retrieved from the AIMDcomputations, a macroscopic scale model of the diffusion controlled uptake ofa powder particle was constructed by coarse graining the time evolution usingthe KMC method.21222. Diffusionally enhancedCO2-over-N2 selectivity in ZeoliteNaKA2.1 Zeolite ALTA-type zeolites are three-dimensional cage type microporous aluminum sil-icates. Belonging to the point group Pm3m, the framework has a cubic peri-odicity built up by so-called - and -cages. Eight (2 2 2) of the larger-cages build up one unit cell (the crystallographic periodic unit) and at theintersections of the -cage corners, the smaller -cages are formed. Hence,each unit cell comprises a combined total of five -cages. Each cage intersectsanother by the pore window rings. The size of the ring number refers to thenumber of O-atoms comprising the ring. Here, the -cages intersect each otherwith 8-rings (8R), the -cages with 4-rings (4R) and the -cages intersect the -cages with 6-rings (6R). As the largest ring size is the 8R, with a diameterof 5, LTA-type zeolites are referred to as narrow pore zeolites since theyonly allow the entrance of small molecules such as CO2 and N2. The 6R and4R pore windows are however too narrow to allow these two gas molecules topass, hence, it is the size of the 8R that determines the uptake. Following this,CO2 and N2 molecules can only enter the space confined by the -cages.Of LTA type zeolites, Zeolite A is the most recognized (Figure 2.1). Thiszeolite is already today intensely used for different industrial, commercial anddomestic applications. For example as catalysts in petroleum refinements [19],for water removal in cat litter and desiccants and for ion exchange in detergents[20]. Zeolite A has an Al-to-Si ratio of 1, which is the highest ratio possible.The Al- and Si-atoms in the framework are strictly alternating in accordancewith Lwensteins rule [21] resulting in a Fm3m symmetry. In turn, this highAl-to-Si ratio leads to a high content of the extra-framework cations, whereeach Al atom is neutralized by one cation valence. In the case of monovalentcations, their are 96 cations per unit cell and for the common case of the Na+cations, the chemical composition is Na96Al96Si96O394 for one unit cell ofZeolite A.These cations are distributed over three types of sites (I, II and III) [2224]238R 4R 6R Zeolite A Unit Cell -cage -cage Figure 2.1: The framework of a Zeolite A unit cell (left) is built up by eight-cages (bottom right). The smaller -cages (top right) are comprised in thecubic intersect of the -cages. The cages are in turn built up by Si-Al-O ringstructures of three different sizes consisting of either four (4R), six (6R) or eight(8R) oxygen atoms. Color key: red=O, yellow=Si, pink=Al.in the plane or centered to one of the three ring types. Site I is centered to the6R, site II is in the plane of the 8R and site III is centered to the 4R. Of these96 extra-framework cations, they will first occupy all 64 6R and 24 8R sitesin the unit cell while the remaining eight cations will be distributed to the 4Rsites, hence, the 4R sites will not be fully occupied. As it is only the 8R thathas a diameter large enough to allow the passage of CO2 or N2, it is the cationoccupying the 8R site, which primarily regulates the passage of these two gasmolecules. The framework containing Na+ ions is referred to as Zeolite NaAor 4A and that containing K+, Zeolite KA or 3A, where 4A and 3A denotes theresulting pore window diameters of approximately 4 and 3 respectively.Zeolite NaKA refers to a mixed Na+ and K+ extra-framework distribution.At the three ion sites Na+ and K+ ions have slightly different positioning asshown in Figure 2.2. At the 4R and 6R sites, K+ protrudes farther from therespective planes due to the larger radius of K+. For the 6R sites Ikeda et al.[24] also showed the occurrence of split sites in Zeolite KA where the K+ ioncan protrude either into the -cage, as for Na+, or into the -cage. At the8R site, both cations position in the 8R plane, however, the smaller Na+ ion24 Figure 2.2: Crystallographic K+ and Na+ positions in Zeolite A. Figure frompaper III.positions off-centre to maximize interaction with two Al-atoms in one of fourgeometrically and energetically equivalent corners while the larger K+ has acentered position interacting with all four Al-atoms in the 8R.2.2 Kinetic molecular sievingIn 1956 Breck et al. [9] performed uptake experiments for small gas moleculesin cation exchanged Zeolite A. These experiments showed that the uptake of acertain gas molecule could be decreased or completely blocked out by chang-ing the type of extra-framework cations. The decreased uptake showed to havea direct relation between the size and shape of the adsorbate molecule and theeffective pore window size of the molecule, which could be tuned by choiceof cation. This was the first demonstration of size selective molecular sieving.Hence, if we are capable of altering the size and shape of the pore windows itshould be possible to enhance the selective properties of zeolites by fine tuningthe size of the pore window openings where one adsorbate type is free to enterwhile another is partially or fully blocked out. This idea has been used widelywhen it comes to separation of hydrocarbons for example [2530]. However,when it comes to separating CO2 from N2, this effect has been scarcely inves-tigated.252.3 Fine-tuning the effective pore window in Zeolite NaKAJust starting my PhD studies, I was introduced to an initial project collabo-ration with the experimental group of Prof. Niklas Hedin. The scope of thisproject was precisely this, to investigate how the CO2-over-N2 selectivity inZeolite A, could be further enhanced by exploiting the difference in kineticdiameters between CO2 and N2 and introduce kinetic separation effects in ad-dition to the already existing thermodynamic separation effects. As the kineticdiameters of CO2 (3.3 ) and N2 (3.6 ) lie right in between the 8R pore di-ameters of Zeolite NaA and KA, most of the CO2 and N2 molecules should beallowed to enter the NaA material and reach thermodynamic equilibrium whilebeing blocked from entering and diffusing through the KA material. Hence,the uptake level of thermodynamic equilibrium cannot be reached in ZeoliteKA.CO2 capacity after the first cycle was related to the presence ofchemisorbed moieties.The IR spectra in Fig. 2 showed that a large fraction of CO2was physisorbed in the NaKA structure for the 0 at.%,17 at.%, and 28 at.% K+ zeolites. The n3 (asymmetric stretching)band at 2346 cm!1, the combination bands (n3 + n1, n3 + 2n2)at 3714 and 3598 cm!1, and the n1 (symmetric stretching) bandat 1381 cm!1 correspond to physisorbed CO2. The symmetricstretching mode of gaseous CO2 is not IR active, but itbecomes detectable as a result of the interaction with thecations. Chemisorbed species were visible in the region18001200 cm!1. These species were assigned as monodentate,bidentate, chelating, or polydentate carbonates.1620 As seen inFig. 2, the quantity of physisorbed CO2 decreased when theK+ content was increased. This decrease agreed with ouradsorption experimental results and IR studies on pure NaAand KA materials.19 For NaA (Fig. 2a), the chelating (1720and 1250 cm!1) and bridged bidentate carbonate (1620 and1362 cm!1) species dominated.19 For small K+ contentzeolites (Fig. 2bc), the bidentate form was dominant. Negativebands are observed at 1175 cm!1. Similar bands have beendetected when CO2 adsorbs on NaA19 and NaY.21 We attributethese negative signals to perturbations of the SiOAlvibrational modes during the adsorption of CO2. The IRspectrum in the chemisorption regime was very different forthe NaKA with the highest K+ content (Fig. 2d). This differenceand the overall low uptake suggested that CO2 adsorbed mainlyon the external particle surface for the K+-rich NaKA. For thissample, the sorption kinetics appeared to hinder the uptake ofCO2 on the timescale of the experiments. We observed thatalmost all physisorbed CO2 can be removed by evacuation forthe NaA, as seen from Fig. 3a. For the NaKA, it was moredifficult to remove CO2 at higher K+ contents. At 17 at.% of K+in NaKA, most physisorbed CO2 could be removed afterapplying dynamic vacuum conditions, only very little CO2remained in the zeolite, see Fig. 3b and S8.w (The IR spectrafor the adsorption and desorption branches on NaKA with17 at.% are presented in the ESI: Figs. S6, S7 and S8.w) Forthe samples with high K+ content, significant amounts ofphysisorbed CO2 remained on NaKA (Fig. 3c and d). Thesedifferent tendencies relate very well with K+ control of the CO2diffusion in NaKA.In order to investigate the regenerability of the zeoliteNaKA, cycle measurements were conducted (Fig. S5w). Theregeneration temperature was an important parameter forzeolite regeneration. In the cycle 4, when the regenerationtemperature decreases to 473 K, the uptake of zeolite NaKAdecreases dramatically. After increasing the temperature to623 K again, the uptake of the sample returns to the highvalue. The decrease of the uptake in cycle 2, cycle 3 and cycle5 is caused by the chemisorption of CO2 on the zeolite.Scheme 1 Illustration of the structural mechanism by which K+reduces the effective pore window aperture in NaKA zeolite.Fig. 1 Uptake of CO2 and N2 (298.15 K, 0.85 bar) in NaKA. Linesare provided to guide the eye.Fig. 2 Infrared spectra of adsorbed CO2 on (a) NaA, and on NaKAwith K+ contents of (b) 17 at.%, (c) 28 at.%, and (d) 88 at.%, at aCO2 pressure of 0.13 bar.Fig. 3 Infrared spectra of adsorbed CO2 on (a) NaA and NaKA withK+ content of (b) 17 at.%, (c) 28 at.% and (d) 88 at.% in thedesorption branch after 1 h evacuation.This journal is "c The Royal Society of Chemistry 2010 Chem. Commun., 2010, 46, 45024504 | 4503Published on 28 April 2010. Downloaded by Stockholms Universitet on 24/10/2014 11:35:02. View Article OnlineFigure 2.3: Schematic illustration of the effective 8R pore diameter of ZeoliteNaKA mechanism resulting from the Na+-to-K+ exchange. Figure from paper I.The idea is that by, in a controlled manner, exchanging the smaller Na+ions for the larger K+ ions, it should be possible to fine tune the materialsfunctionality as a molecular sieve. As illustrated in Figure 2.3, at a certainNa+-to-K+ ratio an effective 8R pore diameter (de f f ) lying right between thekinetic diameters of these two gas molecules, 3.3 < de f f CO2 capacity after the first cycle was related to the presence ofchemisorbed moieties.The IR spectra in Fig. 2 showed that a large fraction of CO2was physisorbed in the NaKA structure for the 0 at.%,17 at.%, and 28 at.% K+ zeolites. The n3 (asymmetric stretching)band at 2346 cm!1, the combination bands (n3 + n1, n3 + 2n2)at 3714 and 3598 cm!1, and the n1 (symmetric stretching) bandat 1381 cm!1 correspond to physisorbed CO2. The symmetricstretching mode of gaseous CO2 is not IR active, but itbecomes detectable as a result of the interaction with thecations. Chemisorbed species were visible in the region18001200 cm!1. These species were assigned as monodentate,bidentate, chelating, or polydentate carbonates.1620 As seen inFig. 2, the quantity of physisorbed CO2 decreased when theK+ content was increased. This decrease agreed with ouradsorption experimental results and IR studies on pure NaAand KA materials.19 For NaA (Fig. 2a), the chelating (1720and 1250 cm!1) and bridged bidentate carbonate (1620 and1362 cm!1) species dominated.19 For small K+ contentzeolites (Fig. 2bc), the bidentate form was dominant. Negativebands are observed at 1175 cm!1. Similar bands have beendetected when CO2 adsorbs on NaA19 and NaY.21 We attributethese negative signals to perturbations of the SiOAlvibrational modes during the adsorption of CO2. The IRspectrum in the chemisorption regime was very different forthe NaKA with the highest K+ content (Fig. 2d). This differenceand the overall low uptake suggested that CO2 adsorbed mainlyon the external particle surface for the K+-rich NaKA. For thissample, the sorption kinetics appeared to hinder the uptake ofCO2 on the timescale of the experiments. We observed thatalmost all physisorbed CO2 can be removed by evacuation forthe NaA, as seen from Fig. 3a. For the NaKA, it was moredifficult to remove CO2 at higher K+ contents. At 17 at.% of K+in NaKA, most physisorbed CO2 could be removed afterapplying dynamic vacuum conditions, only very little CO2remained in the zeolite, see Fig. 3b and S8.w (The IR spectrafor the adsorption and desorption branches on NaKA with17 at.% are presented in the ESI: Figs. S6, S7 and S8.w) Forthe samples with high K+ content, significant amounts ofphysisorbed CO2 remained on NaKA (Fig. 3c and d). Thesedifferent tendencies relate very well with K+ control of the CO2diffusion in NaKA.In order to investigate the regenerability of the zeoliteNaKA, cycle measurements were conducted (Fig. S5w). Theregeneration temperature was an important parameter forzeolite regeneration. In the cycle 4, when the regenerationtemperature decreases to 473 K, the uptake of zeolite NaKAdecreases dramatically. After increasing the temperature to623 K again, the uptake of the sample returns to the highvalue. The decrease of the uptake in cycle 2, cycle 3 and cycle5 is caused by the chemisorption of CO2 on the zeolite.Scheme 1 Illustration of the structural mechanism by which K+reduces the effective pore window aperture in NaKA zeolite.Fig. 1 Uptake of CO2 and N2 (298.15 K, 0.85 bar) in NaKA. Linesare provided to guide the eye.Fig. 2 Infrared spectra of adsorbed CO2 on (a) NaA, and on NaKAwith K+ contents of (b) 17 at.%, (c) 28 at.%, and (d) 88 at.%, at aCO2 pressure of 0.13 bar.Fig. 3 Infrared spectra of adsorbed CO2 on (a) NaA and NaKA withK+ content of (b) 17 at.%, (c) 28 at.% and (d) 88 at.% in thedesorption branch after 1 h evacuation.This journal is "c The Royal Society of Chemistry 2010 Chem. Commun., 2010, 46, 45024504 | 4503Published on 28 April 2010. Downloaded by Stockholms Universitet on 24/10/2014 11:35:02. View Article OnlineFigure 2.4: Experimental CO2 and N2 uptake dependence on the level of Na+-to-K+ exchange at 298.15 K and 0.85 bar. Lines for respective dataset are providedto guide the eye only . Figure from paper I.isotherms for CO2 and N2 were measured at room temperature (298.15 K)up to 0.85 bar for a series of Zeolite NaKA powders with K+/(K++Na+) ratiosvarying from 0 to 1. When plotting the uptakes at 0.85 bar for each structurecomposition as a function of the level of Na+-to-K+ exchange (Figure 2.4) in-teresting behavior was observed. The uptakes for both CO2 and N2 decreasedwith increasing K+-content. This decrease was however non-linear showing adrop in the uptake starting at 10%, for both CO2 and N2. As the N2 uptakestart from an initial low level, the uptake reaches close to zero already at thelevel of 17% Na+-to-K+ exchange. At this level, the CO2 uptake still remainshigh resulting in an exceptionally high selectivity of over 200. This selectivitycan be compared to selectivities of around 10 for similar materials with largepores and without kinetic sieving functionalities for small molecules [3136].When modeling gas adsorption in zeolites, the MMC algorithm in theGrand Canonical ensemble (GCMC) is, more or less, standard use [3746].Hence, the initial approach in paper I to model the adsorption isotherms ofCO2 and N2 in Zeolite NaKA was using this method, which is discussed morein detail in chapter 3. The uptake levels for structure compositions and con-ditions corresponding to those in the experimental setup were simulated andcompared with the experimental data. The modeled levels of uptake were con-27sistently higher than the experimentally measured uptake levels and did notshow the non-linear uptake dependency. Instead, the modeled uptake showed alinear decrease with increasing K+-content. This is a behavior typical for largepore zeolites in which, the extra-framework atoms do not substantially restricta free pore-to-pore diffusion and where the decrease in uptake is mainly theeffect of decreased pore volume resulting from the larger volume of the K+ions compared to Na+ ions [47]. GCMC models the thermodynamic equilib-rium uptake level in a system and cannot describe kinetic effects. Therefore,these results were not surprising and, on the contrary, supported the theoryof kinetic sieving. Here, the thermodynamic effect could not fully describethe non-linear uptake behavior for CO2 and N2 leading to the exceptionallyhigh selectivity measured experimentally in Zeolite NaKA. Hence, in order tomodel a more extensive picture of the uptake it is necessary to take into ac-count the kinetic effects in addition to the thermodynamic effects. This insightinduced the next step, where in paper II, I approached to fully describe theuptake dynamics by combining equilibrium uptake simulations using GCMCwith diffusion simulations using MD.283. Predicting the CO2 uptakeusing force field based modelingIn paper II, I attempted to model the CO2 uptake as a function of the K+-content in the Zeolite NaKA material taking both the thermodynamic as wellas the kinetic effects on the uptake into account. For this, a combination ofclassical modeling methods were used: GCMC to model the equilibrium up-take, predicting the thermodynamic contribution and MD to model the CO2diffusion in the Zeolite structure, predicting the kinetic contribution. Due tothe very slow diffusion of N2 in relation to the timescale accessible to modelwith MD, this study was limited to CO2, hence we could not predict the se-lectivity between these two gas molecules. However, it is not unrealistic toassume that the trends we saw for CO2 in the model are likely to hold trueeven for N2, given a longer time scale. In this case, the high selectivity mea-sured experimentally in paper I could be explained theoretically.Here, I will not go into great detail regarding method theory but insteadfocus on the application of these. Therefore, I would like to refer the inter-ested reader to literature by Frenkel and Smit [48] for a detailed review on thissubject.3.1 Force fieldsWhen performing molecular modeling based on classical mechanics, so-calledclassical modeling methods, the interactions between all particles in the systemare described by a predetermined potential energy model: a distance dependentfunction between two particular particles describing at what distance they repelor attract each other and at what strength. The collection of potential energyor interaction functions for all inter-particle pairs is what is called the systemsforce field. These interaction functions can be divided into two types, eitherdescribing bonded or non-bonded interactions. Bonded interaction functionsinclude a description of the bond vibrations, bond angle bending, and rota-tions around bonds. The non-bonded interaction functions describe the vander Waals and electrostatic interactions.All of these interaction functions are defined by a functional form and29function parameters where the functional form is chosen to best fit the typeof interaction while the function parameters are parameterized to the specificinter-particle interaction. Each particle pair will have a specific set of param-eters, which are parameterized either to fit experimental data (top down ap-proach), derived from quantum chemical calculations (bottom up approach) ora combination of the both.When it comes to classical force field based simulations the accuracy ofthe force field is crucial as it is this that provides the physical substance to themodel. Moreover, in order for a force field based model to be possess predic-tive qualities, it is also necessary that the force field is transferable. Here, trans-ferability implies that the same set of interatomic interaction function shouldbe able to be used for a variety of different molecules of systems other thanthat, which it has been specifically parameterized from. Further, the force fieldshould be able to describe different physical properties, such as thermody-namic interactions as well as diffusion.Unfortunately, a force field describing zeolite-gas interactions living upto both of these requirements in full is, at this point in time, unobtainable.Therefore, when modeling a given physical property for a given system it isnecessary to base the choice of force field on the type of information, whichwe wish to receive and which questions we wish to answer. Is it a qualitativelycomparative study or is quantitative accuracy important?For zeolites, numerous force fields have been developed for interactionwith CO2 and N2, both bottom up and top down, which have high accuracyfor the specific properties and framework they have been parameterized from[38; 39; 4346]. Despite this, I chose to use a force field of generalized type,COMPASS [49] in combination with DFT computed Hirshfeld partial atomiccharges [50]. Generalized force fields are parameterized from a wide rangeof atomic types; elements in different molecular surroundings and not to aspecific system. In general, these generalized force fields are inferior whenit comes to providing high accuracies for specific measurables, however thetransferability is commonly superior.Following this, the choice of force field was based on the following points:1. System specific force fields available for zeolite-gas interactions are gen-erally limited to all-silica zeolites or Na+ containing zeolites. Hence, asystem specific force field for Zeolite NaKA or any K+ containing zeo-lites is not yet available.2. As the objective of this work is to predict the extent, to which the uptakeis facilitated/hindered by thermodynamics and kinetics, respectively, weare looking to avoid a bias where the uptake level is presumed to dependsolely on thermodynamic effects. System specific force field parameters30for zeolite-gas interactions are commonly fitted using GCMC simula-tions to match experimental adsorption isotherms. This approach maybe a good estimation when investigating gas uptake of zeolites withoutsize restricting pores. However, when an unrestricted pore-to-pore dif-fusion of the adsorbate is, to some extent hindered by the size or cationblocking of the pore windows, such as in the case for Zeolite A, the up-take will be affected. In this case, determining a force field by appointingthe full uptake to thermodynamics will create such a bias. Also combi-nations of different force field parameters may give the same outcome,which is apparent when comparing the relatively extensive number ofCO2Zeolite NaA force fields with widely varying parameters for thesame interactions. When modeling specific interactions or quantitiesother than those parameterized from, the outcome may vary greatly be-tween different force fields and, in particular, significant variations inthe outcome of diffusion simulations as shown by Garcia-Sanchz et al.[51].3. As the nature of the study is comparative, i.e. we are looking for trendsrather than absolute values, the transferability weighs stronger than theaccuracy.4. The all-atom COMPASS-force field has a full set of parameters for theCO2 - Zeolite NaKA system containing elaborate models for for boththe bonded and non-bonded interactions. Hence, a fully flexible sys-tem is permitted, which is of particular importance when modeling thediffusion in narrow pore zeolites as the flexibility of the pore windowring and cation may play a crucial role in diffusion. Further, the COM-PASS force field is derived by using ab initio data parameterized from avariety of molecular classes and extensively validated using MolecularDynamics and energy minimizing procedures. A further discussion canbe found in paper II and details regarding the parameters and functionalforms used by the COMPASS force field can be found in the SupportingInformation of paper II.3.2 Modeling the thermodynamic effect with Grand Canon-ical Monte CarloThe Metropolis Monte Carlo algorithm is based purely on statistics and is anefficient method to reach a minimal energy configuration in a system for agiven ensemble by randomly sampling the systems potential energy surfaceaccording to the Boltzmann distribution [12]. We consider a system of atoms31with the potential energy U(r) defined by the applied force field, changingwith U(r) when displacing atoms by . If the move decreases the overallpotential energy of the system the move will be accepted, if not, a randomnumber will be drawn and tested against the Boltzmann distribution of U(r).The algorithm for a MMC step test proceeds as follows:for U =U(r+)U(r)if U 0, accept moveif U > 0, accept move if rnd[0,1] eU/kBTdecline move if rnd[0,1] > eU/kBTThis procedure is iterated until the system is equilibrated, roughly correspond-ing to when the number of accepted moves equal the number of rejected moves.As mentioned in chapter 2, when modeling the uptake of gas adsorbatesin porous materials it is very common to use MMC modeling in the V T orGrand Canonical ensemble, so-called Grand Canonical Monte Carlo (GCMC).In this ensemble the systems chemical potential (), volume (V ) and temper-ature (T ) are held constant while the number of adsorbed molecules (CO2 orN2) to the adsorbent (Zeolite NaKA) is optimized to minimize the system en-ergy and converging into the uptake level of the system at equilibrium. Hence,possible moves for the adsorbate are insertions, deletions, translations and rota-tions. Adsorption isotherms can be modeled by performing a series of GCMCsimulations with stepwise increasing levels of the outside gas pressure regulat-ing the balance between the chemical potential for the gas molecule inside themodeled zeolite system compared to the modeled gas phase.For CO2 and N2 in Zeolite NaKA, the equilibrium uptake is predictedby modeling a series of adsorption isotherms up to 0.85 bar at 298 K withK+/(K++Na+) ratios ranging from 0 to 1 in steps of 0.1. Figure 3.1 showsthe modeled equilibrium uptake together with the experimental uptake frompaper I as a function of the K+/(K++Na+) ratios. As discussed in chapter 2the simulations predict a decrease in the equilibrium uptake with an increas-ing K+-content of the material. This uptake decrease, however, shows a lineardependency deviating from the non-linear experimental uptake dependency.Important to keep in mind, however, is that with GCMC modeling the ki-netic effects are not taken into account as the algorithm, at random, insertsthe adsorbate into the adsorbent in search of the minimum energy configura-tion. Hence, these discrepancies were expected. For large pore zeolites, wherereaching the equilibrium gas uptake is not restricted by diffusional hindrancesof the pore structures, this, method is completely reasonably to predict the to-tal uptake. However, for narrow pore zeolites, such as Zeolite NaKA, taking320 20 40 60 80 10001234K+/(K++Na+) [atom %]Gas uptake [mmol/g]badcFigure 3.1: Uptake of CO2 and N2, experimental values and Grand CanonicalMonte Carlo modeled ones (298.15 K, 0.85 bar) in Zeolite NaKA. Lines forrespective dataset are provided to guide the eye. (a) CO2 sim. (b) CO2 exp. (c)N2 sim. (d) N2 exp. Figure from paper II.into account the kinetic contribution is crucial. Several previous studies, havebeen performed to predict the diffusion of CO2 within the framework of 8-ringzeolites [5254].3.3 Modeling the kinetic effect with Molecular DynamicsTo model the diffusion of CO2 through the Zeolite NaKA material and thereinget a measure of the kinetic contribution to the total uptake, Molecular Dy-namics (MD) is used. These MD simulations are performed in the NV T orCanonical ensemble, where a given number of particles (N) are loaded intothe system with a given volume (V ) at a given temperature (T ), hence theseparameters are held constant through out the MD simulation.In MD the movement of each atom indexed i= 1....N with coordination r ispropagated as a function of time t according the equations of motion followingNewtons second law, Eq. 3.1.d2ridt2=Fimi(3.1)The force Fi acting on atom i at a given time t is equal to the gradient of the33sum of the distance (ri j) dependent interatomic potential functions Nj=1U(ri j)obtained from the applied force field, between atom i and all other atoms inthe system according to Eq. 3.2.5Nj=1U(ri j) = Fi (3.2)This propagation of the atomic motion in the system is performed in dis-crete time steps t, where t is determined system specifically ensuring thatthe fastest motions of relevance are captured and the numerical integration ofthe molecular motions are kept stable. For systems where the fast vibrationalmotion of hydrogen atoms are not of importance, t values of 1-2 fs are com-monly used. For our hydrogen-free system, t is set to 1 fs.Following a time step, the new atomic coordinates of atom i are determinedby solving the equation of motion numerically. Eq. 3.3 shows a simplifiedversion of the truncated Taylor expanded expression.ri(t +t) = ri(t)+vi(t)t +Fi(t)2mit2 (3.3)where the computation of velocity vi(t) depends on the integration algorithmat use.With this approach we can model the movement of the CO2 gas moleculesover time for the different structural compositions of Zeolite NaKA and ob-serve how the increasing K+-content affects the gas molecules ability to dif-fuse through the material and hence, how this could potentially effect the totaluptake. When measuring and comparing the rates of diffusion, it is commonto compute the entity of the self-diffusion coefficient Ds according to Eq. 3.4.Ds =16limtddtNi=1[ri(t) ri(0)]2 (3.4)For CO2 in each of the 11 structural compositions of Zeolite NaKA, Ds wascomputed and plotted as a function of the K+/(K++Na+) ratios and presentedin Figure 3.2. Additionally, Ds was computed for the extra-framework cationsto investigate their behavior as well. As expected, the CO2 diffusion rate de-creased with increasing levels of the larger K+ ions as a result of to the in-creasing number of 8R pores were blocked for the passage of CO2 molecules.However, the observed difference in the mobility of the Na+ and K+ extra-framework cations and how the CO2 diffusion in turn seemingly depended onit, was less expected. The K+ ions showed to have a low mobility, consistentindependently of K+-content of the structure, where the K+ sat comparablyfirmly in their positions unwilling to hop between sites. Na+ on the other340 20 40 60 80 10000.511.52x 106K+/(K++Na+) [atom %]Diffusion Coefficient [cm2/s]CO2Na++K+K+Na+Figure 3.2: Self-diffusion coefficients of CO2, Na+, K+ and N++ K+ combinedin Zeolite NaKA loaded with 52 CO2 molecules/UC, as estimated by NVT-MD.Lines for respective dataset are provided to guide the eye. Figure from paper II.hand, showed a significant mobility between the cation sites in the pure NaAstructure additionally facilitating the CO2 diffusion through Na+ occupied 8Rpore. However, also the mobility of the Na+ ions decreased when the levels ofK+ in the framework increased. This decrease was explained by the increasingnumber of cation sites being occupied by the relatively non-mobile K+, whichleft fewer, energetically favorable, sites for the Na+ ions to hop among. Hence,these simulations predicted that the K+ ions not only effectively block the CO2passage but also restrict the mobility of the Na+ ions, in turn making it moredifficult for CO2 to pass even through the pores occupied by Na+, enhancingthe pore blocking effect at moderate and high levels of Na+-to-K+ exchange.3.4 Predicting the total uptake in narrow pore zeolitesFrom the presented GCMC and MD modeling results of CO2 in Zeolite NaKA,it is clear that both the thermodynamic as well as the kinetic effects contributesubstantially to the total uptake of the varying Zeolite NaKA structure compo-sitions. Hence, when predicting the total uptake in this as well as other narrowpore zeolites, it is necessary to include both these contributions to the model.If we consider the CO2 uptake in a real system such as in an experimentalmeasurement or a PSA/TSA separation process, the uptake cycle is limited intime. In a narrow pore zeolite, such as Zeolite NaAK, with 8R pore diameters35close to the kinetic diameter of the adsorbate, the free diffusion through thematerial will be more or less limited. Hence, it is the adsorbates rate of diffu-sion that will determine the time required to reach the equilibrium uptake leveland for short cycles or slow diffusion, equilibrium will not be reached.Following this reasoning, assuming a direct relation between the extentof freedom that the gas molecules have to diffuse and reach equilibrium, wesimply scale the modeled equilibrium uptake ueq with a correction factor, theroot relative diffusion constantDrels , Eq. 3.5, where D0s corresponds to Ds atthe 0% level of Na+-to-K+ exchange.Drels =(DsD0s) 12(3.5)The total uptake utot is then estimated by scaling the modeled equilibrium up-take values ueq withDrels according to Eq. 3.6.utot =Drels ueq (3.6)We see a substantial improvement to the agreement with the experimental CO2uptake curve in Figure 3.3 when scaling the computed adsorption of CO2 inthis manner.0 20 40 60 80 10001234K+/(K++Na+) [atom %]Gas Uptake [mmol/g]abFigure 3.3: Experimental (a) gas uptakes and combined NVT-MD and GCMCsimulated uptakes according to Eq. 3.6 (b) for CO2 in Zeolite NaKA (0.85 bar,298 K). Lines for respective dataset are provided to guide the eye. Figure frompaper II.364. Predicting the free energybarriers of diffusion usingconstrained AIMD modelingHaving investigated the uptake dynamics of CO2 and N2 in Zeolite NaKAwith classical simulation methods, I had a further interest in investigating thekinetic molecular sieving process in detail and what specific properties effectthe forces and energy barriers of the pore window passages. As force fieldsoften fail to describe specific interactions and dynamics accurately, I chose totake a step down on the multiscale modeling length and time scale (Figure 1.2)to gain accuracy by using constrained ab initio Molecular Dynamics (AIMD).As for the classical method theory, a detailed overview of the theory ofquantum chemistry will not be covered in this thesis as I expect that manyof the readers either already possess this knowledge or do not have sufficientunderstanding of quantum mechanics to follow such an overview, and I do notwish to bore these readers. Also, endless amounts of excellent literature onthe subject already exist and to which, I prefer to refer the interested reader[5557].4.1 Density Functional TheoryQuantum chemical (QC) methods are based on the basic assertion of quan-tum mechanics that the energy E of a system can be retrieved by solving theelectronic Schrdinger equation, Eq. 4.1 [58].H = E (4.1)Here, the hamiltonian operator H, operates on the electronic wave function to yield the ground state system energy provided that describes the elec-tronic structure exactly. However, this deceivingly simple equation hides sev-eral challenging problems, which are addressed in QC computations:1. The Schrdinger equation is impossible to solve analytically and thereinexactly for a system involving more than one electron. Hence, numericalmethods need to be employed.372. Even when using numerical methods it is necessary to apply certain ap-proximations for the many electron problem to be manageable. Themain one being the Born-Oppenheimer approximation [59] assumingto a high accuracy that the nuclei, compared to the electrons, are veryheavy and move on a different time scale than the electrons. This allowsthe nuclei to be treated classically while the electrons are treated withquantum mechanics moving in the field of the fixed nuclei.3. The electronic wave function describing the electronic structure for agiven system is not known exactly. Instead, a set of so-called basis func-tions are used to describe the electron structure for each atom in the sys-tem the atomic orbitals. These basis functions provide the so-calledbasis set. During computations, this basis set is optimized to model thetotal wave function as accurately as possible. In an iterative procedure,the weight of each basis function is optimized to yield the lowest energy.As is known from the variational principle, an arbitrary wave functioncan never yield an energy value lower than the true energy. Followingthis, the weighted combination of functions in a given basis set yield-ing the lowest energy is also the best approximation of the true wavefunction.In Hartree-Fock theory based methods, the problem of solving the manybody wave function is approached directly. Here, the basis functions are com-bined into a trial wave function according to molecular orbital theory, stat-ing that molecular orbitals can be described by a linear combination of theatomic orbitals. Many very evolved and accurate QC computational methodshave been developed from Hartree-Fock theory, however the computationaleffort of using these methods are equally increased. For Hartree-Fock this ef-fort scales by N4, N being the number of electrons in the system, while postHartree-Fock methods such as Configuration Interaction, Coupled-Cluster [60]and Mller-Plesset perturbation theory methods [61] may scale as dramaticallyas N7. Hence, the computational effort of these methods quickly become un-manageable and their use is restricted to small molecular systems.Therefore, Density Functional Theory (DFT) methods [57] have gainedincreasing popularity during the last few decades allowing the treatment oflarger system to a high accuracy. DFT is based on the Hohenberg-Kohn the-orems [62] which, in short, show a mathematical relation between the wavefunction and the electron density. The electron density is described by theKohn-Sham equations [63] treating a fictitious system of non-interacting elec-trons, described by the so-called Kohn-Sham orbitals, where the non-classicalelectron-electron interactions are treated by the electron-correlation functional.Hence, the ground state properties of many-electron systems can be deter-38mined directly from the systems electron density and the handling of the com-putationally impractical many-electron wave function can be avoided. Solvingthe electron density only requires one function of three spatial variables whilesolving the wave function requires three spatial variables for each electron.DFT scales by N3. The DFT approach to solving the molecular electronicstructure is, however, very similar to the Hartree-Fock procedure. The basissets used to describe the Kohn-Sham orbitals and therein the electron den-sity, are optimized iteratively according to the variational principle to find theweighted combination of basis functions yielding the lowest energy, and hencethe best description of the true electron density.The major challenge of DFT lies in the approximation of the electron-correlation functional, which is not known exactly. To date, many functionalsof different complexities have been optimized to treat different problems, ofteninvolving empirical and/or Hartree-Fock information. Also for the case offunctionals, increased complexity entails increased computational effort andthe choice of functional should take into account the functionals suitabilityfor the system and problem under study, accuracy requirements, system sizeas well as the availability of computational resources.An additional drawback of DFT is the theorys insufficient ability to de-scribe van der Waals interactions. This problem is often tackled by an em-pirical correction factor. The most abundantly used van der Waals correctionterms providing reliable results are those developed by Grimme [64].4.2 Periodic DFT-simulations with CP2KAll DFT simulations have been performed using the CP2K software [65].CP2K is an efficient general framework for performing periodic atomistic andmolecular simulations. For DFT simulations, CP2K calculates the DFT forces"on the fly" using the QUICKSTEP module [66; 67], which implements theGaussian and plane waves (GPW) method [68]. This method allows a com-bination of the use of plane-waves describing the electron density with atom-centered Gaussian orbitals representing the wave functions. With this approachboth the computational efficiency as well as accuracy is improved as both dif-fuse and local electrons can be described accurately while using a minimalnumber of basis functions.The QUICKSTEP implementation of the GPW method uses the Goedecker-Teter-Hutter (GTH) pseudopotentials [69] to describe the core electrons as ef-fective core potentials, which is possible as these electrons are generally not in-volved in chemical bonding or polarization. The valence electrons, on the otherhand, are treated explicitly by the DFT and described in our computations byusing the the DZVP-MOLOPT-SR basis set [70]. This Gaussian basis set has39been developed for use with the GTH-pseudopotentials and are augmented bypolarization functions and splitting of the valence to enhance the flexibility inthe description of the valence electrons. To describe the exchange-correlationenergy, the non-empirical Perdew-Burke-Ernzerhof (PBE) functional [71; 72]is used and the van der Waals interactions are described by Grimmes DFT-D3dispersion correction term [64].4.3 Constrained AIMDIn classical MD, the interatomic interactions defining the movement at eachtime step are given by the predefined force field functions as described in Chap-ter 3. However, for AIMD, the interaction forces at each MD step are computeddirectly from the electronic structure by the DFT. Since the DFT does not needspecific parameterization, as is the case for classical molecular dynamics withempirical force fields, the DFT can thus really predict the results. The ma-jor drawback is, however, the comparably high computational effort. Whilefor classical MD, the dynamics of a system consisting of thousands of atomscan easily be modeled on the ns time scale for a reasonable computationalcost, modeling the dynamics with AIMD beyond the ps timescale in a systemof only a few hundred atoms would involve ridiculously huge computationalcosts.Due to this limit in computational time, when using AIMD to investigateevents or transitions between two stable regions, which are not expected tooccur within this window of time, so-called rare events, it is necessary to con-strain the transition coordinates to the path of interest. This constraint method[73; 74] allows a direct estimation of the mean force from the time average ofthe force acting on the geometric constraint. The free energy E can then beestimated by integrating the mean force F(x) as a function of the transitioncoordinates x according to Eq. 4.2.E = x fxiF(x)dx (4.2)Here, the entropy contribution to the free energy barrier comes from the molec-ular movement around the fixed particle.4.4 Determining the free energy barriers of diffusion inZeolite NaKAThe classical MD modeling presented in paper II show that the CO2 moleculein Zeolite NaKA spend the overwhelming majority of the time moving within40the -cage where only approximately every millionth move is through a porewindow and into a new -cage for the case of Na+ 8R occupancy. For thecase of K+ occupancy and for N2 diffusion these occurrences are even morerare. Hence, this pore-to-pore diffusion is a rare-event, which occurs on thens timescale or even longer. As we cannot expect to see this type of transitionwithin the ps timescale, the general limit that can be covered with AIMD, it isnecessary to employ the constraint method presented in the previous section.Following this, in paper III, we present an approach to predict the free en-ergy barriers of diffusion for CO2 and N2 in Zeolite NaKA using constrainedAIMD. This approach is fully expandable to any gas molecule and to any poretype with a diameter close to the kinetic diameter of the gas molecule.d8R plane CO2 COM Figure 4.1: The simulation cell consists of two of the Zeolite A -cage buildingunits. One gas molecule (here CO2) is place in the left -cage and a constraint isset confining the distance d between the geometrical centre of the CO2 moleculeand the 8R window plane intersecting the two cages.To limit the computational effort, the size of the simulation cell is mini-mized to a periodic unit consisting of two intersecting -cages. This is suf-ficient for the purpose of our simulation to investigating the path of the gasmolecules diffusion between these two cages. This simulation cell corre-sponds to 1/4 of a Zeolite A unit cell (Figure 4.1). Also, periodic boundaryconditions (PBC) are imposed, meaning that the simulation cell is reproducedinfinitely. Any particle that exits the left hand side of the cell will enter theright hand side, and so on. The use of PBC avoids problems involved withboundary effects caused by the finite size we are limited to and makes the sys-tem act more like an infinite one. On the other hand, PBC can cause errorsin itself such as periodicity self-image effects i.e. a particle "feels" itself on41the other side of a boundary. This problem is mainly prominent for small sim-ulation cells and despite that our simulation cell is on the lower limit in twodirection (12.3 ) we consider this error to our free energy barrier computa-tions to be negligible since the investigated gas molecule is separated from itsself-image by the zeolite framework and the self-interaction is screened.As the path of interest is the gas molecules movement through the porewindow from one -cage to another the constraint is set to steer the gas moleculethrough the intersecting pore window. This is implemented by using a point-to-plane constraint where the plane is defined by three oxygen atoms in the8R and the point is set to the geometrical centre of the gas molecule as shownin Figure 4.1. This constrains the geometrical centre of the gas molecule tomovement within a parallel plane at this set point-to-plane distance from the8R plane. Hence, allowing unconstrained freedom for the gas molecule tomove in two directions, vibrate and rotate.This point-to-plane distance is stepwise decreased from 4 to 0 (+/- 0.25) with a decreasing step increments; 1 down to 3 , 0.5 down to 1 and0.25 down to 0 . At each step the AIMD was run with a 1.5 fs time step forat least 10 ps, or until the average constraint force had converged to a variationtolerance of 1104 a.u.The average forces are then plotted as a function of the point-to-plane dis-tance and force values are interpolated to a splined smooth force profile. Thefree energy barrier is then estimated by integrating this force profile withinthe free energy barrier region, which is defined to the point-to-plane distanceregion where the force is non-zero and opposing the gas molecules passagethrough the pore. For CO2 passing a Na+ occupied 8R, this region begins at2.5 , while for passing the larger K+ ion it begins already at a distance of4 . Also for the N2 molecules passing both Na+ and K+ occupied 8Rs, theintegration region begins at 4 . This integration region extends to the pointwhere the respective force curve crosses zero, corresponding to the barriersposition at the 8R plane +/- 0.25 .4.5 Identifying the local diffusion rate-determining prop-ertiesUsing the described approach to predict the free energy barriers of diffusion,we seek to identify the systematical rate determining properties of the diffusionfor CO2 and N2 in Zeolite NaKA. In paper IV we systematically go throughspecific environmental variables of the material, which we predict to have arate determining effect and include: cation exchange at the different ion sitesand CO2 loading. These local properties within the simulation cell are altered42accordingly in order to compute how each, respective alternation affects thefree energy barriers of diffusion for CO2 and N2 through the 8R pore.Cation exchangeAs demonstrated in papers I and II, the CO2 and N2 uptake in Zeolite NaKAis strongly affected by the K+-to-Na+-ratio. We expect that the possibility ofpore-to-pore diffusion is mainly dependent on which cation type occupies the8R site as the cation size directly affects the pore window diameter. However,in paper IV the effect of cation exchange in all three sites are investigated and,in fact, show that the impact of the cation composition is a bit more complexthan initially believed.First a "base cell" is defined. This simulation cell unit, as defined in section4.3, is the pure Zeolite NaA structure with no occupied 4R sites neighboringthe pore intersecting 8R window. With this base cell as a starting point, wesystematically go through each site to see how the specific cation occupancyeffects the barrier for the CO2 and N2 diffusion.4R This site does not have full occupancy. According to Rietveld refine-ment powder X-ray diffraction (XRD) experiments [22; 23] only 1/8 of thesesites per -cage are occupied in Zeolite NaA. Hence, there are three situationsto investigate: no ion (base cell), Na+ and K+ occupancy of one of the four 4Rsites neighboring the 8R pore window. It is at this site where the XRD showsthat the Na+-to-K+ exchange occurs first and when the level of Na+-to-K+exchange reaches approximately 8% (8/96) this site is expected to be occupiedonly by K+ ions.8R This site is fully occupied, hence, there are two possible occupanciesof the 8R site in Zeolite NaKA: Na+ (base cell) or K+. Following the exchangeat the 4R sites, the XRD shows that the exchange then occurs predominantlyat the 8R sites. By 40% Na+-to-K+ exchange the 8R sites are expected to befully occupied by K+ ions.6R This site also has full occupancy, hence, the 6R site is either occupiedby Na+ or K+ and there are four fully occupied sites neighboring each 8R,which may effect the diffusion through this pore window. According to theXRD this is the last site to be exchanged.Figures 4.2 and 4.3 show the computed force profiles of CO2 and N2, re-spectively, for the different ion configurations. First, when comparing the re-sults of CO2 and N2 in the base cell, we see that the larger kinetic diameter ofN2 results in a barrier increase of 23% compared to that of CO2. Further, asexpected, it is the occupancy in the 8R site that has the greatest effect on theforce profiles and the resulting free energy barrier for both CO2 and N2. When430 0.5 1 1.5 2 2.5 3 3.5 420246810x 103Pointtoplane distance d [] [a.u.]base cell (35.6)Na 4R (22.6)K 4R (27.4)K 6R (34.4)K 8R (75.0)Figure 4.2: Average force values of CO2 pore-to-pore diffusion for different ionexchange configurations plotted as a function of the distance d between the 8R-plane and geometrical centre of CO2. The computed free energy barrier values,in kJ/mol, are presented in the parenthesis for respective configuration.0.5 0 0.5 1 1.5 2 2.5 3 3.5 420246810x 103Pointtoplane distance d [] [a.u.]base cell (43.9)K+ 4R (43.6) K+ 6R (44.8)K+ 8R (93.3)Figure 4.3: Average force values of N2 pore-to-pore diffusion for different ionexchange configurations plotted as a function of the distance d between the 8R-plane and geometrical centre of N2. The computed free energy barrier values, inkJ/mol, are presented in the parenthesis for respective configuration.44exchanging the Na+ ion to K+ at this position the free energy barrier is morethan doubled resulting from the pore blocking effect of the larger K+ ion.Differences between the two gas molecules are, however, observed for thecation occupation at the 4R site. For CO2, the force curves are significantlyperturbed when a Na+ or K+ ion is added to one of the neighboring 4R sites,resulting in a 37% and 23% decrease of the respective free energy barriers. ForN2, however, the corresponding deviation is 0 0.5 1 1.5 2 2.5 3 3.5 421012345x 103Pointtoplane distance d [] [a.u.]L0, R0 (35.6)L0, R4 (36.0)L4, R0 (34.2)L0, R7 (37.7)L7, R0 (28.1)Figure 4.4: Average force values of CO2 pore-to-pore diffusion for different CO2loadings, in the left and right -cage of the simulation cell, respectively, plottedas a function of the distance d between the 8R-plane and geometrical centre ofCO2. The computed free energy barrier values, in kJ/mol, are presented in theparenthesis for respective configuration.0 1 2 3 4 5 6 78642024Number of loaded CO2E [kJ/mol]Left+right cellLeft cellRight cellFigure 4.5: Extrapolated curve of free energy barrier deviations (E) for CO2loading in the left donor -cage (green) and right acceptor -cage (blue). Thered dashed line shows the sum of the loading effects.46ergy barriers for the different loadings modeled. To see how the CO2 loadingsaffect the free energy barriers, we plot the free energy deviations from the basecell simulation setup as a function of loadings in respective -cage and extrap-olate the intermediate values with a smoothing spline to estimate the trend asshown in Figure 4.5.For the left and the right -cell loadings, we see opposing effects. Whenloading the left donor cage we observe decreased diffusion barriers. This isreasonably explained by the increased gas pressure and number of collisiontowards the diffusing molecule, "helping" it push through the 8R pore. Fol-lowing the same reasoning, an equal, but opposite effect should be observedfrom the loading in the right cage. However, this opposing effect is predictedby the modeling to be smaller. This could be rationalized by the presence ofthe effect proposed by Shang et al. [75] where the interactions between loadedCO2 molecules and the 8R cation facilitate the diffusion through the pore and,in turn, decrease the opposing pressure effect. Hence, this modeling work pre-dicts an increased CO2 loading to have mainly an enhancing effect on the CO2diffusion in Zeolite NaKA.47485. Scaling up: Coarse grainingthe time evolution with KineticMonte CarloLength and time scales involved in experiments are many magnitudes longerthan those possible to achieve with atomistic simulations. Hence, it is oftenquestioned to what extent it is relevant to directly compare and draw conclu-sions regarding dynamical effects probed from microscopic scale models withthose measured with macroscopic scale experiments. However, when model-ing on the atomistic scale, a large portion of the time is often spent on samplingdynamics with little relevance for the macroscopic effects. This is particularlytrue when investigating rare event dynamics, such as in the case for CO2 andN2 diffusion in Zeolite NaKA.In MD, the time step is very short, generally around 1 fs, which is neces-sary to accurately describe the atomistic dynamics. However, as discussed inthe previous chapter the gas molecules spend most of their time moving withina pore, only rarely jumping between pores. When simulating the diffusionon a macroscopic scale, all we really want to know is at what rate do the gasmolecules jump between the pores and through the material. So, given that thepore-to-pore diffusion rates are known, it should be possible to model the dif-fusion through the material based only on this pore-to-pore rate information.Hence as illustrated in Figure 5.1, the intermediate time spent on intra-porediffusion is coarse grained, entailing a substantial computational speed-up.5.1 Kinetic Monte CarloKinetic Monte Carlo (KMC) is a modeling method based on the assertion ofthe Arrhenius rate law [16] that the rate for a given transition between twostates depend on the energy barrier between these states. Instead of samplingthe energy potential landscape in search of the lowest energy state such asin MMC methods, the KMC algorithm evolves the system dynamically fromstate to state according to a given transition state landscape. This dynamicpropagation is however different from that of MD methods in the sense that,49Figure 5.1: Coarse graining the time evolution of the pore-to-pore gas diffusionin Zeolite A.50KMC does not move atoms from one position to another, but instead movesthe system from one state to another.This transition state landscape is defined by all possible transition rates inthe system, or for rare event dynamics, the rates dominating the dynamics. Inour system these are, of course, the pore-to-pore diffusion rates as illustratedtwo-dimensionally in Figure 5.2. Hence, given that the pore-to-pore diffusionrates of our system are known, KMC can preferentially be used to model themacroscopic diffusion of CO2 and N2 through the system as a function oftime. Several previous studies have been performed using the KMC approachto model gas diffusion in zeolites on macroscopic length and time scales [7678]. These studies, however, use force field based MD to predict the pore-to-pore diffusion rates while we approach this from the DFT level of theory.k1 k2 k3 k4 k3 k-3 E3 E-3 Figure 5.2: Given that the pore-to-pore diffusion rates are known for all possibleprocesses, KMC models the gas diffusion through the zeolite by evolving thesystem dynamically from state to state according to the given transition statelandscape.According to the Arrhenius equation [16],k = AeEkBT (5.1)the rate constant k is determined by multiplying the frequency factor A, inter-preted as the number of particles attempting to cross the free energy barrier Eper unit time, with the exponential Boltzmann distribution giving the propor-tion of particles expected to cross E at temperature T . Hence, k is a measureof the number of times per unit time a particle is expected to cross the free51energy barrier and in our case, the number of times per unit time a CO2 or N2molecule is expected to cross a pore window with a given free energy barrier.List all n possible processes k1, k2kn and calculate ktot Pick two random numbers 01, 21 Calculate ki = 1ktot and determine process i to be executed Executed process i and update system Update clock tnew= told+t t = -ln(2)/ktot k1 k2 k3 k4 k5 k6 kn ktot 1ktot Figure 5.3: KMC algorithmFollowing this, the rate constant for a certain transition, referred to as aprocess in the KMC algorithm, has a direct relation to the probability of thattransition occurring. To visualize how the KMC algorithm picks a processto be executed at each step, one can imagine that n one-dimensional vectorswith magnitudes k1,k2...kn for all n possible processes are lined up creatinga total rate vector of magnitude ktot . The process to be executed is chosenstochastically by multiplying a random number 0 < 1 < 1 with ktot . Thisproduct corresponds to a position on the total rate vector, landing on a specificrate constant ki corresponding to process i to be executed. The time incrementt for the KMC step is also determined stochastically by a function of a secondrandom number 0 < 2 < 1 in proportion to the inverse of ktot . Once a processhas been executed, the transition state landscape of the system is then updatedaccording to the new state. This iterative KMC step procedure is describedschematically in Figure 5.3 and for a more detailed description of the KMC52method, excellent reviews by Voter [79], Kratzer [80] and Auerbach [76] canbe recommended.5.2 Determining the rate constantsAccording to Eq. 5.1 the free energy barrier E as well as the frequencyfactor A for temperature T needs to be known for a given transition in order todetermine k. We restrict this study to treat diffusion at room temperature (298K), hence, all computations were performed accordingly.The procedure to retrieve the free energy barriers of diffusion for CO2and N2 from the constrained AIMD computations was already described inchapter 4. The frequency factors A for respective transition are estimated withclassical equilibrium NVT-MD using the same force field and simulation cellas the simulations performed in paper II. These MD simulations are performedon the Zeolite NaA and Zeolite KA structure loaded with one gas moleculeper -cage, both for CO2 and N2 and carried out for 2 ns to collect sufficientstatistics. A is then determined from from each structuregas combination byanalyzing the respective trajectories.Figure 5.4: Two-dimensional illustration of the boarder planes interfacing thefree energy barrier integration region, defined to estimate the pre-exponentialfrequency factors A.As shown in Figure 5.4, planes parallel with each 8R-plane towards thecentre of the pore are defined. The distance between these planes and the8R pore window planes correspond to the point-to-plane distance of the con-strained AIMD computations at where we initiate the integration of the forceprofile to determine the free energy barriers (2.5 or 4.0 ). The number of times53that the gas molecule in each cell passes a border, outwards bound seen fromthe centre of the pore, is counted and the frequency of these occurrences arecomputed. This is an estimation of the frequency at which the gas moleculesattempt to cross the energy barrier, hence an estimation of the frequency factorA. The computed frequency factors are presented in Table 5.1.Table 5.1: Pre-exponential frequency factors A in s1 as computed by NVT-MD.Na+ K+CO2 4.3x1011 9.9x1011N2 4.5x1011 3.5x10115.3 KMC-simulations with KMCLibAll KMC simulations were performed with the KMCLib program [81]. Thissoftware is an efficient general framework for performing lattice KMC simu-lations using the n-fold way algorithm [17] for selecting and executing events.The input to KMCLib is the lattice geometry and site occupation of the start-ing structure and a set of possible processes together with their correspondingrate constants. The output is the lattice site occupations over time, i.e. thetrajectory. Given that the system can be treated as vibrationally equilibrated atthe time an event takes place, and given that all relevant processes and correctrates are provided, the KMC algorithm will describe the correct dynamics ofthe system [18].In order to model the gas dynamics in a porous material this software hasbeen improved to include the possibility of allowing multiple particles on thesame lattice site, as several gas molecules may reside the same cavity. This alsoinvolved modifications to the picking algorithm in order to pick a process at asite with correct probability. These modifications are similar to those describedby Leetmaa and Skorodumova [81] for handling site-specific rates.KMCLib computes the rates "on-the-fly" only recalculating the rates whencorresponding elementary process needs to be updated. This keeps the num-ber of elementary events at a minimum while the necessary flexibility in thedefinition of the rate expressions is withheld.5.4 Modeling the CO2 and N2 uptake in a realistic ZeoliteNaKA powder particle modelThe experimental uptake measurements in paper I were performed on a ZeoliteNaKA powder, where the cubic powder particles were estimated to have an54a = 23 1.23 nm = 28.3 nm a a Figure 5.5: Illustration of the KMC simulation cell set up to model a cubicpowder particle. The simulation cell is built up by 252525 cell units wherethe outer layer models the skin layer adsorption surface and the inner core models232323 -cages.55average diameter of 4 m. To realistically simulate the powder particle, we setup a cubic KMC simulation cell consisting of 252525 cubic cells in paperIV. The outer layer of cells represents a skin layer adsorption surface, whilethe inner core represents 232323 -cages. This gives us a simulation cellwith cell parameters of a = b = c = 23 12.3 = 28.3 nm shown in Figure5.5. Further, as the uptake rate is expected to scale quadratically, we scale thesimulation time accordingly (4106 m/28.3109 m)2 = 2104 in orderto compare the KMC simulations with the experimental results. In each cellfour lattice sites are defined: one gas site and three ion sites. The gas sites arelocated in the centre of each cell, constituting the lattice for the dynamics of thegas diffusion and in the centre of the x, y and z cell-to-cell intersecting plane,respectively, the ion sites are located. The ion sites define the combination ofcations in and around the 8R pore, which determine the pore-to-pore diffusionrate, either on its own or in addition to the number of gas molecules occupyingthe gas sites involved. The skin layer gas sites allow adsorption and diffusionto a first layer -cage while the -cage gas sites allow diffusion between -cages. The ion site occupations were held constant during the simulations andwere distributed randomly according to the ion compositions for each modeledlevel of Na+-to-K+ exchange as presented in Tables 5.2 and 5.3 for CO2 andN2, respectively.Table 5.2: Cation distribution in % for different Zeolite NaKA structure compo-sitions for KMC model of CO2 diffusion.K+/(K++Na+) 0 0.08 0.17 0.33 0.50 0.67 0.83 18R=Na+ 67 67 44 0 0 0 0 08R=Na+, 4R=Na+ 33 0 0 0 0 0 0 08R=Na+, 4R=K+ 0 33 22 0 0 0 0 08R=K+ 0 0 23 67 69 75 86 08R=K+, 4R=K+ 0 0 11 33 31 25 14 100Table 5.3: Cation distribution in % for different Zeolite NaKA structure compo-sitions for KMC model of N2 diffusion.K+/(K++Na+) 0 0.07 0.13 0.20 0.27 0.338R=Na+ 100 80 60 40 20 08R=K+ 0 20 40 60 80 100For CO2, only the combination of the 8R and 4R occupations are considered asthe 6R occupations did not show to affect the free energy barriers of CO2 pore-to-pore diffusion significantly. For N2, only the distribution of 8R occupationsare considered as neither the 4R or 6R occupation showed a significant effect56on the pore-to-pore diffusion of N2.The KMC simulations are principally a measure of the kinetic uptake de-pendence and do not take into account the aspect of the uptake dependence onthe thermodynamic equilibrium. Hence, an uptake cap per cell unit is definedaccording to the equilibrium uptake levels predicted by the GCMC uptake sim-ulations in paper II and is set to the upper integer number of gas molecules per-cage for the respective level of Na+-to-K+ exchange.When all 4R and 8R ions are exchanged to K+ at levels higher than 33%Na+-to-K+ exchange, CO2 the uptake should not drop significantly beyond alinear decrease following the decrease of the equilibrium uptake since the Na+-to-K+ exchange at the 6R site does not substantially effect the free energy bar-riers. As a possible explanation to the drastic decrease at higher levels of Na+-to-K+ exchange seen experimentally, we suggest that the weakly bound 4R K+ions may prefer a split 6R occupancy for certain ion configurations, resultingin a decrease in populated 4R sites at high levels of Na+-to-K+ exchange. Us-ing the same computational setup as for the AIMD simulations, non-dynamicalDFT geometry optimizations were performed to investigate this. We tested thestability of the K+ occupation in the 4R site for three different starting config-urations:1. K+ occupied 4R with both neighboring 6Rs occupied by Na+-ions2. K+ occupied 4R with one neighboring 6R occupied by a Na+-ion andthe other by a K+-ion3. K+ occupied 4R with both neighboring 6Rs occupied by K+-ionsFor cases (1) and (2) the K+ ion was stable in the 4R site while for case (3) theion relaxed to one of the neighboring 6R sites resulting in a doubly occupied6R. At 50% Na+-to-K+ exchange, 1/4 of the 6R sites are expected to be oc-cupied by K+ ions, at 67% 1/2, at 87% 3/4 and at 100% the 6R sites are fullyoccupied by K+. The number of K+ in the 6R sites surrounding a specific8R is expected to follow the binomial distribution determining the proportionof K+ ions preferring the split 6R over the 4R, hence reducing the number ofK+ occupied 4Rs accordingly. These proportions have been considered whendetermining the combination of ion compositions for the KMC simulations aspresented in Table 5.2.5.5 Testing the effects of rate-determining propertiesIn paper IV, we test the macroscopic effect of the cation exchange and theloading as predicted to be rate determining by previous studies [22; 53; 75; 8284] and by our free energy barrier computations. Additionally, we test the rate57determining effect of the presence of skin layer surface defects blocking theentrance into the inner volume of the material. This has been suggested byCheung et al. [85] to have a significant effect on the adsorption kinetics. Asadsorption is an exothermic process, the adsorption to the skin layer should notin itself limit the diffusion and uptake of the gas molecules. However, if onlya portion of the skin layer act as entrance channels into the bulk, the uptakewill be significantly restricted. Figures 5.6 and 5.7 show the KMC modeleduptakes testing these different effect for CO2 and N2, respectively, togetherwith the corresponding experimental data from paper I.For CO2 we present three different curves modeling the uptake after 1 hourin addition to the experimental curve:0 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9 100.511.522.533.544.5K+/(K++Na+)CO2 uptake [mmol/g]excl. loading effectsincl. loading effectsincl. loading effects,incl. 75% surface defectsExperimentalFigure 5.6: KMC modeled CO2 uptake after 1 hour plotted as a function of thelevel of Na+-to-K+ exchange for the three different simulation setups: exclud-ing effects of CO2 loading (blue), including effects of CO2 loading (green) andincluding the effects of CO2 loading and including 75% surface defects (red).These are compared to the experimental data from paper I (cyan). Lines areprovides to guide the eye only.1. The blue curve in Figure 5.6 shows the KMC modeled uptake depen-dency on the level of cation exchange. Here, the effect of the CO2loading on the free energy barriers have not been taken into accountwhen computing the various pore-to-pore diffusion rates. We see a goodcorrespondence with the experimental data at low levels of Na+-to-K+exchange due to the fast adsorption kinetics where the equilibrium capuptake levels are reached within a matter of seconds or minutes. ForNa+-to-K+ exchange levels of 33% and higher, the equilibrium cap isnot reached within the 1 hour time limit as all the 8R sites are now oc-cupied by K+ ions. This drastically decreases the rates of diffusion.58Hence, we see a substantial drop in the uptake, which is in correspon-dence with that seen experimentally, however, at moderate to high levels(33%-83%) of cation exchange the modeled uptake levels are overesti-mated by 25-30% compared to experiments.2. The uptake presented by the green curve in Figure 5.6 includes the effectof the CO2 loadings predicted by the computed free energy barriers asshown in Figure 4.5. As the loading, in total, increases the pore-to-pore diffusion rates, the effect is mainly an acceleration of the uptakerate resulting in an additional increase of the uptake at moderate to highlevels of cation exchange. This results in an increase of the deviationbetween the modeled uptake and experimental uptake to 35-100%.3. For the uptake data presented by the red curve in Figure 5.6, 75% ofthe skin layer cells of the powder particle model have been blocked foradsorption, hence, modeling the effect of skin layer surface defect poreblocking. These modeled defects decrease the uptake rate and the levelof uptakes reached after 1 hour for moderate to high loadings are broughtto an excellent agreement with the experimental values.For N2 we present the following three modeled curves, showing uptakesafter 1 hour in addition to the experimental curve:1. As for CO2, the blue curve in Figure 5.7 shows the KMC modeleduptake dependency on the level of cation exchange. Here, the uptakeat low loadings is overestimated by 100% or more. This is an arti-fact of the equilibrium cap being restricted to an integer number of N2molecules/-cage. Here, the cap is set to 1/-cage while the equilibriumlevel is estimated to ca. 0.5/-cage for the pure NaA structure composi-tion and decreasing for increasing levels of Na+-to-K+ exchange.2. The green curve in Figure 5.7 shows the KMC modeled uptake scaledby the GCMC equilibrium levels enabling a qualitative comparison withthe experimental uptake levels. This curve shows a sharp uptake dropstarting at 15% Na+-to-K+ exchange and reaching zero uptake at 25%.This is a slight deviation from the experimental curve showing the cor-responding drop between 5% and 15% Na+-to-K+ exchange.3. The red curve in Figure 5.7 shows the scaled, modeled uptake including75% skin surface defects. The applied defects contribute to a slight im-provement towards an agreement with the experimental data by shiftingthe uptake drop region to 10-20% Na+-to-K+ exchange.590 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9 100.10.20.30.40.5K+/(K++Na+)N2 uptake [mmol/g]Modeled uptakeScaled to eq. uptakeScaled to eq. uptake,incl. 75% surface defectsExperimentalFigure 5.7: KMC modeled N2 uptake after 1 hour plotted as a function of thelevel of Na+-to-K+ exchange for the three different simulation setups: no scaling(blue), scaled to fit equilibrium uptake levels (green) and scaled to fit equilibriumuptake levels and including 75% surface defects (red). These are compared to theexperimental data from paper I (cyan). Lines are provides to guide the eye only.5.6 Adsorption kineticsAs discussed in the recent papers by Cheung et al. [85] and Akhtar et al. [86],the adsorption kinetics of the CO2 uptake plays an important role for potentialindustrial applications. For an efficient swing adsorption process rapid uptakedynamics are necessary where cycle times < 5 minutes are sought. Followingthis reasoning, Akhtar et al. [86] presented a figure of merit taking into accountthe CO2-over-N2 selectivity and level of CO2 uptake within a time limit of 1minute, for the purpose of rating a materials performance as a sorbent. Ac-cording to this figure of merit, Zeolite NaKA with 10% Na+-to-K+ exchangeshows the best performance experimentally due to a fast uptake rate despitea lower CO2-over-N2 selectivity compared to the 17% Na+-to-K+ exchangelevel. Figure 5.8 shows the KMC modeled uptake for CO2 and N2 uptake after1 minute. These results show a high selectivity at 8% Na+-to-K+ exchangewhile still reaching a high level of CO2, 99% of the equilibrium level. Hence,our results concure with those of Akhtar et al. showing that a lower level ofNa+-to-K+ exchange is preferential when taking adsorption kinetics into ac-count.However, when comparing the simulated time required to reach the max-imum uptakes for 0% and 17% Na+-to-K+ exchange levels with the experi-mental uptake times presented by Cheung et al. [85], we see that the modeledadsorption kinetics are significantly faster. The simulations show that 90%600 0.1 0.2 0.3 0.4 0.5 0.6 0.7 0.8 0.9 100.511.522.533.544.5K+/(K++Na+)CO2/N2uptake [mmol/g] CO2N299% CO2 uptakeCO2/N2=142Figure 5.8: KMC modeled CO2 and N2 uptake after 1 minute plotted as a func-tion of the level of Na+-to-K+.of the maximum uptake is reached in 0.3 and 3 seconds, respectively, whilethe experiments show that corresponding uptakes take as long as 22 and 125seconds. This indicates that additional rate limiting effects are likely to havesignificant effects. Such factors as internal surface defects, heat transfer fromthe the exothermic surface adsorption and presence of water have been sug-gested to potentially affect the uptake dynamics in otherwise similar crystalsand conditions [85; 87] and should be interesting to investigate in future work.61626. Conclusions and OutlookThis thesis has focused on describing the process of kinetic sieving for CO2-over-N2 separation in Zeolite NaKA with a multiscale modeling approach. Wehave used several different modeling methods employing various levels of the-ory to describe and explain this molecular sieving process on different lengthand timescales, extending from the electronic scale to the macroscopic scale.In paper I, we showed that the widely used GCMC method for modelinggas uptake in nanoporous materials is not sufficient when the systems possi-bility of reaching equilibrium within a given cycle time is hindered by kineticconstriction of the pores.In paper II, the experimental uptake dependence of CO2 on the level ofK+-to-Na+ exchange in the Zeolite NaKA material could be qualitatively re-produced by combining the GCMC modeled equilibrium uptake levels withthe kinetic effects modeled by MD diffusion simulations. These results gavefurther support to the theory of a diffusion enhanced selectivity proposed inpaper I, stating that it is the kinetic effects that really distinguishes this systemfrom others similar systems, which depend solely on thermodynamic effects.Additionally, this classical modeling work suggested that the difference in mo-bilities of the different cation types may play a role in the sieving capability inthis and similar materials.Taking a more detailed and quantitative approach to describe the pore-to-pore diffusion process of CO2 and N2 through different pore types, whilebypassing problems involved with the use of force fields, paper III presents aprocedure to estimate the free energy barriers of diffusion using constrainedAIMD. These computed free energy barriers show that the CO2 and N2 dif-fusion through a cation occupied 8R is, in fact, a rare event with a higherbarrier for the kinetically larger N2 molecule compared to CO2. Additionally,the computations show Na+-to-K+ relative transition rates in the magnitude of104. This conveys a negligible probability of pore-to-pore diffusion through aK+ occupied 8R explaining the zero uptake of both CO2 and N2 in Zeolite KAshown in experiments.Using the constrained AIMD approach presented in paper III to computethe free energy barriers of diffusion we, in paper IV, seek to identify the localproperties in the Zeolite NaKA pore, which determine the pore-to-pore diffu-sion rates of CO2 and N2. In particular, we investigate the role that the different63cation occupancies in the different sites play on the free energy barrier as wellas the effect of the presence of additional CO2 molecules in the pore the CO2loading. We show that for CO2 the occupation of the 4R site plays a significantrole for the diffusion by lowering the barrier, while for the more inert N2 nosuch effect is detected. Further, this free energy barrier information is used asinput for the KMC simulations, where we on a macroscopic scale predict thediffusion driven uptake, enabling a direct comparison with the experiments.With KMC we model the effects, of the cation exchange, CO2 loading andpresence of skin layer surface defects. Additionally, we suggest a model bycombining these effects, showing an excellent agreement with the experimen-tal uptake data for CO2 and N2 from paper I. This temporal coarse grainingapproach takes electronic scale information to a macroscopic level and is aviable method to test the macroscopic scale effects of microscopic propertieswhile, to a large extent, bypassing the use of force field based simulation meth-ods (Figure 6.1). With constrained DFT-MD the free energy barriers of diffusion for gas molecules in porous molecular sieves can be determined accurately. This allows us to identify the rate determining properties of the molecular sieve for the a gas molecule. The free energy barriers from the DFT-MD simulations can be used directly into the KMC algorithm allowing us to simulate the diffusion of the gas molecules through the material up to microsecond timescales or even longer. This information is important insight when designing new highly selective materials for the purpose of gas separation with temperature/pressure swing capture processes, where employing kinetic aspects is likely to further increase energy efficiency of swing technologies for carbon capture and separation in addition to the more elaborately investigated equilibrium-based separation. Coarse Graining the Time Evolution with Kinetic Monte Carlo4 F(d) F(d) = E Ae/kBT = k Calculating Energy Barriers with Constrained DFT- MD The Blue Moon Ensemble3,4 Temporal Coarse Graining for Gas Diffusion in Small Pore Zeolites From the Quantum Scale to the Macroscopic Introduction1,2 Conclusions Amber Macea, Mikael Leetmaab, Niklas Hedina, Kari Laasonenc and Aatto Laaksonena aBerzelii Center EXSELENT on Porous Materials, Department of Materials and Environmental Chemistry, Stockholm University, Sweden bDepartment of Physics and Astronomy, Uppsala University, Sweden. cDepartment of Chemistry, Aalto University, Finland References 1Liu, Mace, Bacsik, Sun, Laaksonen, Hedin, Chem. Comm. 2010, 46, 4502-4504 2Mace, Hedin, Laaksonen, J. Phys. Chem. C 2013, 117, 24259-24267 3Mace Laasonen, Laaksonen, Phys. Chem. Chem. Phys. 2014, 16, 166-172 4Mace, Leetmaa, Hedin, Laaksonen, Unpublished work in progress. +Zeolites with 8-ring window apertures, such as those of Zeolite A (LTA), coinciding with the approximate size of small gaseous molecules are interesting candidates for selective gas adsorbents with swing adsorption technologies due to their potential molecular sieving capabilities. We are investigating computationally how the CO2-over-N2 selectivity in LTA-type materials can be greatly enhanced by altering properties of the material, such as through cation exchange or variation of the Si/Al-ratio. To map how the sieving capabilities are affected by these alternations we use DFT based molecular dynamics (DFT-MD) to predict how the free energy barriers of diffusion are affected when altering the composition of the framework. This information can then be used to simulate the macroscopic (>s) diffusion of these gas molecules by using the Transition State Theory based method: Kinetic Monte Carlo (KMC). The mean force F(d) acting on the gas molecule can directly be estimated from the force on the geometric constraint. The free energy of diffusion is then retrieved by integrating the force profile from the center of the cell to the pore window plane (d=6-0). d 8R plane CO2 COM As diffusion from one pore to another is a rare event, the gas molecule needs to be gu ided through the pore window. This is done with a distance constraint between the plane of the pore window and the gas molecule. k1 k2 k3 k4 From the free energy barrier of diffusion E of a specific process p, the diffusion rate k is determined giving the probability of that specific event occurring in the KMC step. Determine all possible processes p for givensystem configuration and build a list.Get all rate constantskpGet two random numbers 1 , 2 ]0,1]Calculate ktot = p kpand find process q:q q-1kp 1 ktot kpp=1 p =1Execute process number q,i.e. update configurationupdate clockt t ln( 2)/ktotSTARTEND0ktot1 ktotqFIG. 3: Flow chart illustrating the basic steps in the rejection-free BKL algorithm. The loop starts with the determinationof all processes (and their rate constants) that are possiblefor the current system configuration. After the generationof two random numbers, the system is advanced accordingto the process selected by the first random number and thesystem clock increments according to the computed total rateconstant and the second random number, as prescribed byan ensemble of Poisson processes. Thereafter the loop startsanew, or the simulation is terminated, if a sufficiently longtime span has been covered.different pathways given by the different rate constants.Each pathway has thus its own probability distributionfunction for the time of first escape. Say, if we are cur-rently in state i, we have for each possible pathway toanother state j a Poisson distributionpij(t) = kij exp (kijt) . (4)Since only one event can be the first to happen, an in-tuitive generalization to propagate the kMC trajectory,also known as the first-reaction method18, would be todraw a random number for each possible pathway andtherewith determine for each one of them an exponen-tially distributed escape time through an expression ofthe form of Eq. (3). We then pick the pathway withthe shortest escape time, move the system to the statereached by that pathway, advance the system clock bythe corresponding shortest escape time, and begin againfrom the new state. Even though this is a perfectly validkMC algorithm, it is clearly not particularly efficient, aswe have to draw a lot of random numbers to generate allthe different escape times and then discard all but one ofthem.Among a variety of numerically efficient kMC algo-rithms suggested in the literature19,20, the one most com-monly used in practice is often attributed to Bortz, Kalosand Lebowitz21 even though one can clearly trace its ideaback further8. As such, it is sometimes referred to as theBKL algorithm, with the N -fold way, residence-timealgorithm or Gillespie algorithm being other frequentlyemployed names. Figure 3 compiles a flowchart of this al-gorithm. As necessarily required in any kMC procedure,it starts with the determination of all N possible pro-cesses, aka escape pathways, out of the present systemconfiguration, aka state. The corresponding N differentrate constants are then summed to yield the total rateconstantktot =Np=1kp . (5)Executed is the process q, which fulfills the conditionqp=1kp 1ktot q1p=1kp , (6)where 1 ]0, 1] is a random number. In order to un-derstand the idea behind this condition imagine for eachprocess p a block of height kp. If we then stack all ofthese blocks on top of each other as illustrated in Fig. 3,we arrive at a stack of total height ktot. Choosing a ran-dom height along this stack, i.e. 0 < 1ktot ktot, willpoint to one of the blocks and this is the process that isselected. Obviously, a process with a large rate constant,i.e. a large block height, has a higher chance of beingchosen in this way, and this probability weighted selec-tion is precisely what the partial sums in Eq. (6) achieve.By executing the selected process the system is moved tothe new configuration, the system clock is advanced byt t ln(2)ktot, (7)where 2 ]0, 1] is another random number, and the en-tire cycle starts anew from the new system state. Insteadof drawing N different random numbers for the N pos-sible pathways as in the intuitive first-reaction method,this algorithm thus needs only two in each cycle, whichin case of realistic systems of the type discussed belowmakes a huge computational difference. Each cycle fur-thermore definitely propagates the system to a new state,which is also often viewed as an advantage of the corre-sponding class of rejection-free kMC algorithms.An important aspect of the BKL algorithm is that thetime by which the clock is advanced, cf. Eq. (7), isindependent of which process was actually chosen. Tounderstand this it is important to realize that the overallscale of tescape is governed by the fastest process thatcan occur in a given configuration. This process withthe highest rate constant has the shortest average escapetime, cf. Eq. (4), and even in the maybe more intuitivefirst-reaction method a slower process has only a chanceof getting selected if its randomly drawn escape time is ofthis order of magnitude. Since the Poisson distribution ofthis slower process is centered around a longer average es-cape time, this happens only rarely and correspondinglythe slow process occurs less often than the fast ones inthe generated kMC trajectory as should be the case. InKMC-algoritm scheme borrowed from: First-Principles Kinetic Monte Carlo Simulations for Heterogeneous Catalysis: Concepts, Status and Frontiers by Karsten Reuter With KMC we dont care about what happens within the pores we are only interested in the probablilties that a gas molecule from pore to another. As the gas molecule spends most of its time moving within the pore, one KMC move is equivalent to millions of MD moves. This enables simulations up to macroscopic time scales, which can make it possible to compare with experiments and predict diffusion properties in such materials. 10-15 10-12 10-9 10-6 10-3 1 time(s) KMC length(m) 10-9 10-6 10-3 DFT-MD FF-MD MD-trajectory Coarse grained KMC-trajectory This approach allows us to identify the systematical rate determining properties of the diffusion in the molecular sieve, including exchange of cations at specific sites, the Si/Al ratio of the framework and the loading of CO2. We observe that the CO2 molecule is strongly affected by variations of the local structure while N2 is much less so. However, for both CO2 and N2, the main rate determining property is the cation species occupying the 8R pore window site, which is the path of diffusion. PBC: 2x1x1 -cages 0 1 2 3 420246810x 103d [Angstrom]F [a.u.]Na+ 4R (22 kJ/mol)Na+ 8R (30 kJ/mol)K+ 8R (74 kJ/mol)K+ 4R (26 kJ/mol)K+ 6R (24 kJ/mol)CO20 1 2 3 420246810x 103d [Angstrom]F [a.u.]Na+ 8R (43 kJ/mol)K+ 8R (84 kJ/mol)K+ 4R (41 kJ/mol)K+ 6R (42 kJ/mol)N2Figure 6.1: Modeling methods used in this thesis treating different levels of thelength and time scale.This procedure should be possible to apply when investigating the kineticsof any guest molecule in any porous material where the pore-to-pore diffusioncan be defined as a rare event. The KMC-model as implemented by KMClib isvery flexible, allowing any number of individual processes and interdependent64dynamics of different types. This opens up for complex models to simulate re-alistic situations. Such a model setup could consist of several different phaseswith different dynamic behavior combined with a magnitude of different localenvironment dependent processes in addition to macroscopic condition varia-tions. For example, the presence of temperature gradients effecting the transi-tion rates depending on where in the material the process takes place such asillustrated in Figure 6.2.Gas phase Surface adsorption First layer entrance Bulk diffusion T=298 K, P=1 atm Temperature gradient Figure 6.2: Example of different phases and effects, which could be added to aKMC model.Currently, we are computing the free energy barriers for the site-to-sitehopping of Na+ and K+ ions in Zeolite A, using a similar approach as forpore-to-pore gas diffusion. In the near future we, hence, plan to extend ourKMC model to investigate the effects of the cation mobilities. Additional fu-ture studies should involve a continued investigation to identify and test theeffects of additional, potentially rate determining effects using this approach.Such additional properties interesting to investigate involve internal surfacedefects, temperature effects and presence of water. On a broader scale, dy-namical effects of the variations of pore size, shape and flexibility are highlyinteresting to investigate as well as expanding the study to include other typesof extra-framework cations and other gas molecules. By collecting barrier in-formation on a large number of different pore window apertures and gases,this information can be combined in many different ways to model a specificzeolite-gas system on a macroscopic timescale based mainly on informationwith a quantum chemical accuracy.Despite the exceptionally high CO2-over-N2 selectivity measured for Ze-olite NaKA, there is one major drawback for this material when it comes to65applicability in an industrial separation process, namely the fact that ZeoliteA is strongly hydrophilic. For water containing flue-gases, this will involvea significant uptake of water, resulting in a decreased CO2 uptake due to thepreferential adsorption of the highly polar water molecule. Following this, onemight ask why then we are studying this material. This material has showedvery interesting properties when it comes to the phenomenom of kinetic molec-ular sieving and how it can be tuned by ion exchange. By studying this materialwe have gained insight to the properties, which effect this process and tunabil-ity. With gained knowledge on how these processes work we are more adept todevelop new or identify existing materials with similar molecular sieving qual-ities but with lower or less competitive uptake of water. This knowledge maybe conclusive in the attempt to lower the "parasitic energy" for carbon captureand separation processes. Such materials, which have been studied for thispurpose, with more or less success, are certain Aluminum phosphates (AlPOs)[88] and Silica aluminum phosphates (SAPOs) [89] in addition to the ZeoliteNaKA with Si-to-Al ratios > 1, so-called ZK-4 [90]. Of these mentioned, thelatter is also subject for an ongoing modeling work showing particularly in-teresting behavior as the decreased number of negatively charged Al-atoms inthe framework decrease the energy potential wells in the cation sites, in turn,increasing the cation mobilities, which may show to have a further effect onthe gas dynamics.66Sammanfattning p svenskaEnligt en stor majoritet av de ledande klimatforskarna utgr den pgende glo-bala uppvrmingen ett reellt hot mot mnsklighetens vlbefinnande p jorden.Det finns starka vetenskapliga bevis att denna uppvrmning r ett direkt resul-tat av den kraftiga kningen av utslpp av vxthusgaser, i synnerhet CO2, somfljer frbrnningen av fossila brnslen ssom olja och kol som skett undersenaste rhundradet. Fr att bromsa den negativa klimatutvecklingen behverCO2 utslppen minska drastiskt p kort tid. Att utveckla effektiva metoder fratt separera och fnga upp CO2 frn industriella avgaser r drmed en ndvn-dighet. Det r ven avgrande att dessa metoder r kostnadseffektiva fr attskerstlla en bred anvndning ven i utvecklingslnder dr kolfrbrnning rden huvudsakliga energikllan.Zeoliter r nanoporsa kristallina material uppbyggda av periodiska ram-verk bestende av kisel-, aluminium- och syreatomer. Porsiteten ger materi-alet en omfattande inre ytarea p vilken gasadsorption (bindning p yta) kanske. Denna egenskap har gjort zeoliter till ett srskilt intressant material frindustriell CO2 separation d de kan attrahera stora mngder CO2 molekyleroch sedan till en relativt lg energikostnad slppa dessa igen genom att varieratemperaturen eller gastrycket i systemet. Materialet kan drmed teranvndas.Vid separationen av CO2 frn N2, som utgr huvudkomponenten av kolfr-brnningsavgaser, r det tv huvudsakliga skillnader hos dessa tv molekylersom kan utnyttjas i processen. Fr det frsta r CO2 mer reaktiv jmfrt medden relativt inerta N2 molekylen. Detta r framfrallt p grund av att det s.k.kvadrupolmomentet r nstan tre gnger hgre hos CO2, vilket gr att den haren starkare attraktionskraft till materialytan. Fr det andra har CO2 moleky-len en lite mindre s.k. kinetisk diameter vilket gr att den kan ta sig genomlite mindre zeolitporppningar jmfr med N2. D den kinetiska separationenkan ses som en passiv process, finns potential att ka kostnadseffektivitetenhos industriella separationsprocesser om material med sdana molekylra fil-treringsegenskaper kan komma till nytta.Zeoliter av LTA-typ r uppbyggda av tredimensionella porer med por-ppningar som sammanfaller med storleksordningen hos CO2 och N2, 3-5 (1010m). Genom att variera jontypen som sitter i porppningen, r det mjligtatt ven justera materialets funktion som molekylrt filter, dr mlet r att CO2molekylerna fritt ska kunna trnga sig in i porerna fr adsorption, medan destrre N2 molekylerna blockeras. Fr Zeolit NaKA (LTA-typ zeolit innehllan-de Na+ och K+ joner) uppns en exceptionellt hg CO2-ver-N2 selektivitet.Under de senaste rtiondena har molekylr modellering tagit en alltmerframtrdande roll i forskningen av molekylra system. Fr materialforskninghar modelleringen blivit en integrerad och viktig del av analysen och mjlig-heten att frutse ett materials fysiska och kemiska egenskaper d en insyn pmolekylr-, atom- och t.o.m. elektronniv mjliggrs.Fr att noggrant kunna modellera separationsprocessen behvs en kvant-kemisk beskrivning av systemet dr den kemiska upplsningen r p elektron-niv. Men fr industriella applikationer r det framfrallt nskvrt att kunnafrutse processen p en makroskopisk skala. Drmed r flerskalig modelle-ring en ndvndighet fr att beskriva den molekylra filtreringsprocessen i sinhelhet.I denna avhandling anvnds ett flertal modelleringmetoder som behandlarolika lngd- och tidsskalor fr att beskriva den kinetiska separationen av CO2frn N2 i Zeolit NaKA. I ett frsta steg anvnds en kombination av klassisk-mekaniska kraftfltsmetoder fr att visa vikten av att inkludera bde effekternaav de termodynamiska attraktionskrafterna svl som kinetiska effekter vidmodellering av gasadsorptionen i zeoliter dr gasdiffusionen i ngon grad rhindrad av trnga porppningar.Fr att sedan ge en ytterligare detaljerad bild av gasmolekylernas dynamikgenom materialet, introducerar vi en modelleringsprocedur fr att berkna des.k. fria energibarrirerna som begrnsar gasfldet mellan porerna. Denna pro-cedur som baseras p kvantkemisk molekyldynamik anvnder vi fr att iden-tifiera vilka lokala egenskaper hos porerna som pverkar hur enkelt det r frgasmolekylerna att frflytta sig genom Zeolit NaKA-materialet. De poregen-skaper som vi undersker innefattar kombinationen av Na+ och K+ joner polika krystallografiska positioner inom materialet samt nrvaron av ytterligareCO2 molekyler inne i porerna.Informationen om hur energibarrirna pverkas av de olika lokala miljer-na inom porerna infogas i Kinetisk Monte Carlo (KMC) metoden som anvndsfr att simulera och jmfra pverkan av dessa och andra effekter, p den kine-tiska filtreringen och gasupptaget i en realistisk Zeolit NaKA pulverpartikel-modell, p en makroskopiska tidsskala. Drmed skalar vi upp information somerhllits direkt frn noggranna kvantkemiska berkningsmetoder med en upp-lsning p elektronniv till en makroskopisk skala. Detta mjliggr en direktjmfrelse mellan modelleringsresultat och experiment samt en frutsgelseav pverkan av olika materialegenskaper p industriella applikationer.AcknowledgementsDuring my PhD studies at the Department of Materials and EnvironmentalChemistry I have had the pleasure to cross roads with many very intelligent,creative, motivated and otherwise great people who have in one way or an othercontributed to my development as a scientist and a person.First and foremost, my gratitude goes to my supervisor Prof. Aatto Laak-sonen for opening up important doors for me while providing me with thefreedom and encouragement to follow my own path and develop an indepen-dence crucial for a future successful research career. To my co-supervisor,Prof. Niklas Hedin, I owe particular appreciation. Your patience, hard workand chemical intuition has inspired me deeply and I am very fortunate to havebeen given the opportunity to collaborate with you and your group. My deepestgratitude also goes to Prof. Arnold Maliniak and Prof. Jozef Kowalewski foralways being supportive and stable points, particularly in times of frustration.During my PhD I have had many great collaborations, several directly con-tributing to this thesis and have been important guides in my PhD roadmap anddevelopment of ideas. Of course, thanks to Qingling, Zoltan B. and Niklas forbringing me me into the world of kinetic molecular sieving and Zeolite NaKA.Great thanks goes to Prof. Kari Laasonen for introducing me to the AIMDmethods allowing my thesis work to take new dimensions. I really learnt alot from you. I am also very thankful for the most recent collaboration withMikael Leetmaa. Without your interest, motivation and great software KM-Clib, the resulting KMC work would not have been possible.I have also been particularly fortunate to have been given the opportunity totake part in several additional project collaborations outside of my thesis work.Of course, this work and collaborations have equally contributed to broadeningmy knowledge and scientific development. Alexander Larin, your drive is ina league of its own, thank you for sharing it with me. Shichao and Mats, Ireally enjoyed working with you as well as getting the opportunity to studylone pair and ELF structures. Thank you, Ilich and Xiadong for bringing meinto the exciting world of MOFs. Ilich, it is really stimulating to collaboratewith someone so excited about his work, and mine! Neda and Lennart, thankyou for dragging me outside of my CO2 bubble, and into the world of other,more smelly, adsorbates! Ocean and Panagiotis thanks for great discussionsand collaboration its been NaKA ok! (I apologize for my poor sense ofhumor.)There are also many wonderful people in my surrounding which, in dif-ferent ways, have had great impact on my time at MMK and SU. Thank youArnold, Jozef, Jon, Baltzar, Sasha L. and Erik for great lunches, debating any-thing and everything from heaven to earth. We dont always agree, but I alwaysappreciate the discussions and different viewpoints. I am very fortunate to havehad so many great colleagues, whom I also consider friends. Jon, I am partic-ularly happy to have had you to share teaching duties and PhD representationwork with. Its been great working with someone who is equally motivated inaddition to having great personal qualities such as always being calm, rationaland thorough. Sasha M., thank you for being such a good roommate, always sokind, considerate and happy to help, even when it comes to answering "stupid"questions regarding Python. And Neda, I am very happy to have found a friendin such a genuine person. Yonglei, Joakim, Zoltan T., Fransesca, Henrik. F.,Samrand, Tom, Linna, Mikaela, Miia, Alexandra and so many more have indifferent ways enhanced my time at the department.During my PhD time, I have dedicated a large portion of my efforts to PhDrepresentation work on the department, faculty as well as central level. Thiswork has been immensely instructive and stimulating and I have been veryfortunate to meet so many great people on this journey. I would like to thankeveryone working with me over the years in the Department board, PhD coun-cil, Faculty board and council, University Board as well as different workinggroups. In particular, I would like to acknowledge all the talented and moti-vated people in CDR including Fredrik C. L. for great work and discussions.I would also like to thank Gunnar S. for keeping an encouraging, benevolentand open mindset.Without the endless love, help and support of my family I would never bewhere I am today. To my Mother, Father, Brothers and In-laws, I owe all ofyou boundless appreciation for always being there for me. Annabelle, thankyou for keeping my priorities straight by showing me what is really importantin life. This has provided we with the personal distance to my work, whichI believe to be crucial for success. Andreas, I honestly do not know what Ihave done to deserve you and how you put up with my stubbornness. But, I doknow that I am extremely lucky to have you and I am deeply grateful for everysecond with you and everything you do for me and our family. Thank you. Ilove you.References[1] WORKING GROUP II. Climate Change 2014: Impacts, Adaption and Vulnerability. Technicalreport, Intergovernmental Panel on Climate Change (IPCC), New York, 2014. 15[2] WORKING GROUP I. Climate Change 2013: The Physical Science Basis. Technical report, Inter-governmental Panel on Climate Change (IPCC), New York, 2013. 15[3] WORKING GROUP III. IPCC Special Report on Carbon Dioxide Capture and Storage. Technicalreport, Intergovernmental Panel on Climate Change (IPCC), New York, 2005. 15[4] S. CHAKRAVARTI, A. GUPTA, AND B. HUNEK. Advanced Technology for the Capture of CarbonDioxide from Flue Gases. First National Conference on Carbon Sequestration, 2001. 15[5] D. AARON AND C. TSOURIS. Separation of CO2 from Flue Gas: A Review. Sep. Sci. Technol.,40:321348, 2005. 15[6] R. T. YANG. Adsorbents: Fundamentals and Applications. John Wiley & Sons, Inc., New Jersey,2003. 16[7] L.-C. LIN, A. H. BERGER, R. L. MARTIN, J. KIM, J. SWISHER, K. JARIWALA, C. H. RYCROFT,A. S. BHOWN, M. W. DEEM, M. HARANCZYK, AND B. SMIT. In Silico Screening of Carbon-capture Materials. Nature Materials, 11:19, 2012. 16[8] C. GRAHAM, D. A. IMRIE, AND R. E. RAAB. Measurement of the electric quadrupole momentsof CO2, CO, N2, Cl2 and BF3. Mol. Phys., 93:4956, 1998. 17[9] D. W. BRECK. Zeolite Molecular Sieves. Wiley & Sons, 1974. 18, 25[10] G. E. MOORE. Cramming more components onto integrated circuits. Electronics, 38:114117,1965. 18[11] Nobel Prize Scientific Background on the Nobel Prize in Chemistry 2013: Development of mul-tiscale models for complex chemical systems. 19[12] N. METROPOLIS, A. W. ROSENBLUTH, M. N. ROSENBLUTH, A. H. TELLER, AND E. TELLER.Equation of State Calculations by Fast Computing Machines. J. Phys. Chem., 21:10871092,1953. 19, 31[13] B. J. ALDER AND T. E. WAINWRIGHT. Studies in Molecular Dynamics. I. General Method. J.Chem. Phys., 31:459466, 1959. 19[14] A. RAHMAN. Correlations in the Motion of Atoms in Liquid Argon. Phys. Rev. A, 136:405411,1964. 19[15] L. G. DUNFIELD, A. W. BURGESS, AND H. A. J. SCHERAGA. Energy Parameters in Polypep-tides. 8. Empirical Potential Energy Algorithm for the Conformational Analysis of LargeMolecules. Phys. Chem., 82:26092616, 1978. 21http://www.ipcc.ch/report/ar5/wg2/http://www.ipcc.ch/report/ar5/wg1/http://www.ipcc-wg3.de/special-reports/special-report-on-carbon-dioxide-capture-and-storagehttp://www.alrc.doe.gov/publications/proceedings/01/carbon_seq/p9.pdfhttp://www.alrc.doe.gov/publications/proceedings/01/carbon_seq/p9.pdfhttp://www.tandfonline.com/doi/abs/10.1081/SS-200042244http://www.nature.com/nmat/journal/v11/n7/full/nmat3336.htmlhttp://www.nature.com/nmat/journal/v11/n7/full/nmat3336.htmlhttp://www.tandfonline.com/doi/abs/10.1080/002689798169429http://www.tandfonline.com/doi/abs/10.1080/002689798169429http://www.nobelprize.org/nobel_prizes/chemistry/laureates/2013/advanced-chemistryprize2013.pdfhttp://www.nobelprize.org/nobel_prizes/chemistry/laureates/2013/advanced-chemistryprize2013.pdfhttp://scitation.aip.org/content/aip/journal/jcp/21/6/10.1063/1.1699114http://scitation.aip.org/content/aip/journal/jcp/31/2/10.1063/1.1730376http://journals.aps.org/pr/abstract/10.1103/PhysRev.136.A405http://pubs.acs.org/doi/abs/10.1021/j100513a014http://pubs.acs.org/doi/abs/10.1021/j100513a014http://pubs.acs.org/doi/abs/10.1021/j100513a014[16] S. A. ARRHENIUS. ber die Reaktionsgeschwindigkeit bei der Inversion von Rohrzucker durchSuren. Z. Physik. Chem., 4:266, 1889. 21, 49, 51[17] A. B. BORTZ, M. H. KALOS, AND J. L. LEBOWITZ. A New Algorithm for Monte Carlo Simula-tions of Ising Spin Systems. J. Comput. Phys., 17:1018, 1975. 21, 54[18] K A. FICHTHORN AND W. H. WEINBERG. Theoretical foundations of dynamical Monte Carlosimulations. J. Chem. Phys., 95:10901096, 1991. 21, 54[19] J. WEITKAMP AND L. PUPPE. Catalysis and Zeolites: Fundamentals and Applications. Springer-Verlag, Berlin, 1999. 23[20] R. P. TOWNSEND AND E. N. COKER. Ion exchange in zeolites. Stud. Surf. Sci. Catal., 137:467524,2001. 23[21] W. LWENSTEIN. The distribution of aluminum in the tetrahedra of silicates and aluminates.Am. Mineral., 39:9296, 1954. 23[22] Q. LIU, A. MACE, Z. BACSIK, J. SUN, A. LAAKSONEN, AND N. HEDIN. NaKA sorbents withhigh CO2-over-N2 selectivity and high capacity to adsorb CO2. Chem. Comm., 46:45024504,2010. 23, 43, 57[23] J. J. PLUTH AND J. V. SMITH. Accurate Redetermination of Crystal Structure of DehydratedZeolite A. Absence of Near Zero Coordination of Sodium. Refinement of Silicon, Aluminum-Ordered Superstructure. J. Am. Chem. Soc., 102:47044708, 1980. 43[24] T. IKEDA, T. KODAIRA, T. OH, AND A. NISAWA. K+ ion distribution in zeolite ZK-4s with vari-ous Si/Al ratios and the contribution of K+ ions to K cluster formation. Microporous MesoporousMater., 57:249261, 2002. 23, 24[25] R. SCHOELLNER AND U. MUELLER. Influence of mono- and bivalent cations in 4A-zeoliteson the adsorption separation of ethene and propene from crack-gases. Adsorpt. Sci. Technol.,3:167171, 1986. 25[26] Y. T. YEH AND R. T. YANG. Diffusion in Zeolites Containing Mixed Cations. AIChE J., 35:16591666, 1989.[27] S. U. REGE, J. PADIN, AND R. T. YANG. Olefin/Paraffin Separations by Adsorption: -complexation vs. Kinetic Separation. AIChE J., 44:799809, 1998.[28] J. PADIN, S. U.; REGE, R. T. YANG, AND L. S. CHENG. Molecular-Sieve Sorbents for KineticSeparation of Propane/Propylene. Chem. Eng. Sci., 55:45254535, 2000.[29] M. MAES, L. ALAERTS, VERMOORTELE F., R. AMELOOT, S. COUCK, V. FINSY, J. F. M. DE-NAYER, AND D. E. DE VOS. Separation of C5-Hydrocarbons on Microporous Materials: Com-plementary Performance of MOFs and Zeolites. J. Am. Chem. Soc., 132:22842292, 2010.[30] C. A. GRANDE, A. LIND, . VISTAD, AND D. AKPORIAYE. Olefin-Paraffin Separation UsingCalcium-ETS-4. Ind. Eng. Chem. Res., 53:1552215530, 2014. 25[31] M. P. BERNAL, M. CORONAS, M. MENNDES, AND J. SANTAMARA. Separation of CO2/N2Mixtures Using MFI-type Zeolite Membranes. AIChE J., 50:127135, 2004. 27[32] R. V. SIRWARDANE, M. S. SHEN, AND E. FISHER. Adsorption of CO2 on Zeolites at ModerateTemperatures. Energy Fuels, 19:11531159, 2005.[33] T. Q. GARDNER, A. I. FLORES, R. D. NOBLE, AND J. L. FALCONER. Transient Measurementsof Adsorption and Diffusion in H-ZSM-5 Membranes. AIChE J., 48:11551167, 2002.http://www.sciencedirect.com/science/article/pii/0021999175900601http://www.sciencedirect.com/science/article/pii/0021999175900601http://scitation.aip.org/content/aip/journal/jcp/95/2/10.1063/1.461138http://scitation.aip.org/content/aip/journal/jcp/95/2/10.1063/1.461138http://www.sciencedirect.com/science/article/pii/S0167299101802536http://www.minsocam.org/ammin/AM39/AM39_92.pdfhttp://www.ncbi.nlm.nih.gov/pubmed/20428579http://www.ncbi.nlm.nih.gov/pubmed/20428579http://pubs.acs.org/doi/abs/10.1021/ja00534a024http://pubs.acs.org/doi/abs/10.1021/ja00534a024http://pubs.acs.org/doi/abs/10.1021/ja00534a024http://www.sciencedirect.com/science/article/pii/S1387181102005954http://www.sciencedirect.com/science/article/pii/S1387181102005954http://onlinelibrary.wiley.com/doi/10.1002/aic.690351010/abstracthttp://onlinelibrary.wiley.com/doi/10.1002/aic.690440405/abstracthttp://onlinelibrary.wiley.com/doi/10.1002/aic.690440405/abstracthttp://www.sciencedirect.com/science/article/pii/S0009250900000993http://www.sciencedirect.com/science/article/pii/S0009250900000993http://pubs.acs.org/doi/abs/10.1021/ja9088378http://pubs.acs.org/doi/abs/10.1021/ja9088378http://pubs.acs.org/doi/abs/10.1021/ie00022a002http://pubs.acs.org/doi/abs/10.1021/ie00022a002http://onlinelibrary.wiley.com/doi/10.1002/aic.10012/fullhttp://onlinelibrary.wiley.com/doi/10.1002/aic.10012/fullhttp://pubs.acs.org/doi/abs/10.1021/ef040059hhttp://pubs.acs.org/doi/abs/10.1021/ef040059hhttp://onlinelibrary.wiley.com/doi/10.1002/aic.690480604/abstracthttp://onlinelibrary.wiley.com/doi/10.1002/aic.690480604/abstract[34] P. J. E. HARLICK AND F. H. TEZEL. Adsorption of Carbon Dioxide, Methane and Nitrogen:Pure and Binary Mixture Adsorption for ZSM-5 with SiO2Al2O3 ratio of 280. Sep. Pur. Technol.,33:199210, 2003.[35] T. HASEGAW, K. WATENABE, K KUSAKABE, AND S. MOROOKA. The Separation of CO2 UsingY-type Zeolite Membranes Ion-exchanged with Alkali Metal Cations. Sep. Pur. Technol., 2223:319325, 2001.[36] K. KUSAKABE, T. KURODA, K. UCHINO, Y. HASEGAWA, AND S. MAROOKO. Gas PermeationProperties of Ion-exchanged Faujasite-type Zeolite Membranes. AIChE J., 45:12201226, 2004.27[37] E. JARAMILLO AND M. CHANDROSS. Adsorption of Small Molecules in LTA Zeolites. 1. NH3,CO2, and H2O in Zeolite 4A. J. Phys. Chem. B, 108:2015520159, 2004. 27[38] E. D. AKTEN, R. SIRIWARDANE, AND D. S. SHOLL. Monte Carlo Simulation of Single- andBinary-component Adsorption of CO2, N2, and H2 in Zeolite Na-4A. Energy Fuels, 17:977983,2003. 30[39] G. MAURIN, P. L. LLEWELLYN, AND R. G. BELL. Adsorption Mechanism of Carbon Dioxide inFaujasites: Grand Canonical Monte Carlo Simulations and Microcalorimetry Measurements.J. Phys. Chem. B, 109:1608416091, 2005. 30[40] R. S. PILLAI, S. A. PETER, AND R. V. JASRA. Correlation of Sorption Behavior of Nitrogen,Oxygen, and Argon with Ca2+ Locations in Zeolite A: A Grand Canonical Monte Carlo Simu-lation Study. Langmuir, 23:88998909, 2007.[41] G. MAURIN, Y. BELMABKHOUT, G. PIRNGRUBER, L. GABEROVA, AND P. LLEWELLYN. CO2Adsorption in LiY and NaY at High Temperature: Molecular Simulations Compared to Exper-iments. Adsorption, 13:453460, 2007.[42] B. SMIT AND T. L. M. MAESEN. Molecular Simulations of Zeolites: Adsorption, Diffusion, andShape Selectivity. Chem. Rev., 108:41254184, 2008.[43] A. GARCA-SNCHEZ, C. O. ANIA, J. B. PARRA, D. DUBBELDAM, T. J. H. VLUGT, R. KR-ISHNA, AND S. CALERO. Transferable Force Field for Carbon Dioxide Adsorption in Zeolites.J. Phys. Chem. C, 113:88148820, 2009. 30[44] M. FISCHER AND R. G. BELL. Influence of Zeolite Topology on CO2/N2 Separation Behavior:Force-Field Simulations Using a DFT-Derived Charge Model. J. Phys. Chem. C, 116:2644926463, 2012.[45] H. FANG, P. KAMAKOTI, J. ZANG, S. CUNDY, C. PAUR, P. I. RAVIKOVITCH, AND D. S. SHOLL.Prediction of CO2 Adsorption Properties in Zeolites Using Force Fields Derived from PeriodicDispersion-Corrected DFT Calculations. J. Phys. Chem. C, 116:1069210701, 2012.[46] H. FANG, P. KAMAKOTI, P. I. RAVIKOVITCH, M. ARONSON, C. PAUR, AND D. S. SHOLL. Firstprinciples derived, transferable force fields for CO2 adsorption in Na-exchanged cationic zeo-lites. Phys. Chem. Chem. Phys., 15:1288212894, 2013. 27, 30[47] R. D. SHANNON. Revised Effective Ionic Radii and Systematic Studies of Interatomic Distancesin Halides and Chalcogenides. Acta Cryst. A, 32:751767, 1976. 28[48] D. FRENKEL AND B. SMIT. Understanding Molecular Simulation. Academic Press, 2002. 29[49] H. SUN. COMPASS: An ab Initio Forcefield Optimized for Condensed-Phase Application-Overview with Details on Alkane and Benzene Compounds. J. Phys. Chem. B, 102:73387364,1998. 30http://www.sciencedirect.com/science/article/pii/S1383586602000783http://www.sciencedirect.com/science/article/pii/S1383586602000783http://www.sciencedirect.com/science/article/pii/S1383586600001544http://www.sciencedirect.com/science/article/pii/S1383586600001544http://onlinelibrary.wiley.com/doi/10.1002/aic.690450608/abstracthttp://onlinelibrary.wiley.com/doi/10.1002/aic.690450608/abstracthttp://pubs.acs.org/doi/abs/10.1021/jp048078fhttp://pubs.acs.org/doi/abs/10.1021/jp048078fhttp://pubs.acs.org/doi/abs/10.1021/ef0300038http://pubs.acs.org/doi/abs/10.1021/ef0300038http://pubs.acs.org/doi/abs/10.1021/jp052716shttp://pubs.acs.org/doi/abs/10.1021/jp052716shttp://pubs.acs.org/doi/abs/10.1021/la700821nhttp://pubs.acs.org/doi/abs/10.1021/la700821nhttp://pubs.acs.org/doi/abs/10.1021/la700821nhttp://link.springer.com/article/10.1007/s10450-007-9038-0http://link.springer.com/article/10.1007/s10450-007-9038-0http://link.springer.com/article/10.1007/s10450-007-9038-0http://pubs.acs.org/doi/abs/10.1021/cr8002642?journalCode=chreayhttp://pubs.acs.org/doi/abs/10.1021/cr8002642?journalCode=chreayhttp://pubs.acs.org/doi/abs/10.1021/jp810871fhttp://pubs.acs.org/doi/abs/10.1021/jp3099768http://pubs.acs.org/doi/abs/10.1021/jp3099768http://pubs.acs.org/doi/abs/10.1021/jp302433bhttp://pubs.acs.org/doi/abs/10.1021/jp302433bhttp://pubs.rsc.org/en/content/articlelanding/2013/cp/c3cp52246fhttp://pubs.rsc.org/en/content/articlelanding/2013/cp/c3cp52246fhttp://pubs.rsc.org/en/content/articlelanding/2013/cp/c3cp52246fhttp://scripts.iucr.org/cgi-bin/paper?s0567739476001551http://scripts.iucr.org/cgi-bin/paper?s0567739476001551http://pubs.acs.org/doi/abs/10.1021/jp980939vhttp://pubs.acs.org/doi/abs/10.1021/jp980939v[50] F. L. HIRSHFELD. Bonded-atom Fragments for Describing Molecular Charge Densities. Theor.Chim. Acta, 44:129138, 1977. 30[51] A. GARCA-SNCHEZ, J. VAN DEN BERGH, J. M. CASTILLO, S. CALERO, F. KAPTEIJN, ANDT. J. H. VJUGT. Influence of force field parameters on computed diffusion coefficients of CO2in LTA-type zeolite. Microporous Mesoporous Mater., 158:6476, 2012. 31[52] R. KRISHNA AND J. M. VAN BATEN. A Molecular Dynamics Investigation of a Variety of In-fluences of Temperature on Diffusion in Zeolites. Microporous Mesoporous Mater., 125:126134,2009. 33[53] R. KRISHNA AND J. M. VAN BATEN. A Molecular Dynamics Investigation of the DiffusionCharacteristics of Cavity-type Zeolites with 8-Ring Windows. Microporous Mesoporous Mater.,137:8391, 2011. 45, 57[54] L. MADISON, H. HEITZER, C. RUSSELL, AND D. KOHEN. Atomistic Simulations of CO2 and N2within Cage-type Silica Zeolites. Langmuir, 27:19541963, 2011. 33[55] A. SZABO AND N. S. OSTLUND. Modern Quantum Chemistry. Dover Publications Inc., 1996. 37[56] I. N. LEVINE. Quantum Chemistry. Prentice Hall, 1991.[57] R. G. PARR AND W. YANG. Density-Functional Theory of Atoms and Molecules. Oxford UniversityPress, 1989. 37, 38[58] E. SCHRDINGER. An Undulatory Theory of the Mechanics of Atoms and Molecules. Phys. Rev.,28:10491070, 1926. 37[59] M. BORN AND R. OPPENHEIMER. Zur Quantentheorie der Molekeln. Ann. Phys., 84:457484,1927. 38[60] J. CZEK. On the Correlation Problem in Atomic and Molecular Systems. Calculation of Wave-function Components in Ursell-Type Expansion Using Quantum-Field Theoretical Methods. J.Chem. Phys., 45:42564266, 1966. 38[61] C. MLLER AND M. S. PLESSET. Note on an Approximation Treatment for Many-ElectronSystems. Phys. Rev., 46:618622, 1934. 38[62] P. HOHENBERG AND W. KOHN. Inhomogeneous electron gas. Phys. Rev. B, 136:864871, 1964.38[63] W. KOHN AND L. J. SHAM. Self-consistent equations including exchange and correlation effects.Phys. Rev. A, 140:11331138, 1965. 38[64] S. GRIMME, J. ANTONY, S. EHRLICH, AND H. KRIEG. A consistent and accurate ab initioparametrization of density functional dispersion correction (dft-d) for the 94 elements H-Pu. J.Chem. Phys., 132:154104154119, 2010. 39, 40[65] CP2K, version 2.4.0, 2013. 39[66] M. KRACK AND M. PARRINELLO. Quickstep: Make the atoms dance. NIC Series, 25:2951,2004. 39[67] J. VANDEVONDELE, M. KRACK, F. MOHAMED, M. PARRINELLO, T. CHASSAING, AND J. HUT-TER. Quickstep: fast and accurate density functional calculations using a mixed Gaussian andplane waves approach. Comp. Phys. Comm., 167:103128, 2005. 39[68] G. LIPPERT, J. HUTTER, AND M. PARINELLO. The Gaussian and augmented-plane-wave densityfunctional method for ab initio molecular dynamics simulations. Theor. Chem. Acc., 103:124140,1999. 39http://link.springer.com/article/10.1007%2FBF00549096http://www.sciencedirect.com/science/article/pii/S1387181112001588http://www.sciencedirect.com/science/article/pii/S1387181112001588http://www.sciencedirect.com/science/article/pii/S1387181109000389http://www.sciencedirect.com/science/article/pii/S1387181109000389http://linkinghub.elsevier.com/retrieve/pii/S1387181110002775http://linkinghub.elsevier.com/retrieve/pii/S1387181110002775http://pubs.acs.org/doi/abs/10.1021/la104245chttp://pubs.acs.org/doi/abs/10.1021/la104245chttp://journals.aps.org/pr/abstract/10.1103/PhysRev.28.1049http://onlinelibrary.wiley.com/doi/10.1002/andp.19273892002/abstracthttp://scitation.aip.org/content/aip/journal/jcp/45/11/10.1063/1.1727484http://scitation.aip.org/content/aip/journal/jcp/45/11/10.1063/1.1727484http://journals.aps.org/pr/abstract/10.1103/PhysRev.46.618http://journals.aps.org/pr/abstract/10.1103/PhysRev.46.618http://journals.aps.org/pr/abstract/10.1103/PhysRev.136.B864http://journals.aps.org/pr/abstract/10.1103/PhysRev.140.A1133http://scitation.aip.org/content/aip/journal/jcp/132/15/10.1063/1.3382344http://scitation.aip.org/content/aip/journal/jcp/132/15/10.1063/1.3382344http://www.cp2k.org/http://webarchiv.fz-juelich.de/nic-series/volume25/volume25.htmlhttp://www.sciencedirect.com/science/article/pii/S0010465505000615http://www.sciencedirect.com/science/article/pii/S0010465505000615http://link.springer.com/article/10.1007%2Fs002140050523http://link.springer.com/article/10.1007%2Fs002140050523[69] S. GOEDECKER, M. TETER, AND J. HUTTER. Separable dual-space Gaussian pseudopotentials.Phys. Rev. B, 54:17031710, 1996. 39[70] J. VANDEVONDELE AND J. HUTTER. Gaussian basis sets for accurate calculations on molecularsystems in gas and condensed phases. J. Chem. Phys., 127:114105114113, 2007. 39[71] J. P. PERDEW, K. BURKE, AND M. ERNZERHOF. Generalized Gradient Approximation MadeSimple. Phys. Rev. Lett., 78:38653868, 1996. 40[72] J. P. PERDEW, K. BURKE, AND M. ERNZERHOF. Erratum: Generalized Gradient Approxima-tion Made Simple. Phys. Rev. Lett., 78:1396, 1996. 40[73] M. SPRIK AND G. CICCOTTI. Free energy from constrained molecular dynamics. J. Chem. Phys.,109:77377744, 1998. 40[74] E. A. CARTER, G. CICCOTTI, J. T. HYNES, AND R. KAPRAL. Constrained reaction coordinatedynamics for the simulation of rare events. Chem. Phys. Lett., 156:472477, 1989. 40[75] J. SHANG, G. LI, R. SINGH, Q. GU, K.M. NAIRN, T.J. BASTOW, N. MEDHEKAR, C. M. DO-HERTY, A. J. HILL, J. Z. LIU, AND P. A. WEBLEY. Discriminative Separation of Gases by a"Molecular Trapdoor" Mechanism in Chabazite Zeolites. J. Am. Chem. Soc., 136:1924619253,2012. 47, 57[76] S. AUERBACH. Theory and simulation of jump dynamics, diffusion and phase equilibrium innanopores. Int. Rev. Phys. Chem, 19:155198, 2000. 51, 53[77] R. KRISHNA AND J. M. VAN BATEN. Kinetic Monte Carlo Simulations of the Loading Depen-dence of Diffusion in Zeolites. Chem. Eng. Technol., 28, 2005.[78] M. K. F. ABOUELNASRA AND B. SMIT. Diffusion in Confinement: Kinetic Simulations of Self-and Collective-diffusion Behavior of Adsorbed Gases. Phys. Chem. Chem. Phys., 14:1160011609,2013. 51[79] A. VOTER. Introduction to the Kinetic Monte Carlo Method. NATO Science Series, 235:123,2007. 53[80] P. KRATZER. Monte Carlo and Kinetic Monte Carlo Methods - A Tutorial. NIC Series, 42:5176,2009. 53[81] M. LEETMAA AND N. V. SKORODUMOVA. KMCLib: A general framework for lattice kineticMonte Carlo (KMC) simulations. Comput. Phys. Commun., 185:23402349, 2014. 54[82] R. D. BRECK, W. G. EVERSOLE, R. M. MILTON, T. B. REED, AND T. L. THOMAS. CrystallineZeolites. I. The Properties of a New Synthetic Zeolite, Type A. J. Am. Chem. Soc., 78:59635971,1956. 57[83] A. MACE, N. HEDIN, AND A. LAAKSONEN. Role of Ion Mobility in Molecular Sieving of CO2over N2 with Zeolite NaKA. J. Phys. Chem. B, 117:2425924267, 2013.[84] A. MACE, K. LAASONEN, AND A. LAAKSONEN. Free energy barriers for CO2 and N2 in zeoliteNaKA: an ab initio molecular dynamics approach. Phys. Chem. Chem. Phys., 16:166172, 2014.57[85] O. CHEUNG, Z. BACSIK, Q. LIU, A. MACE, AND N. HEDIN. Adsorption kinetics for CO2 onhighly selective zeolites NaKA and nano-NaKA. Applied Energy, 112:13261336, 2013. 58, 60,61[86] F. AKHTAR, Q. LIU, N. HEDIN, AND L. BERGSTRM. Strong and binder free structured zeolitesorbents with very high CO2-over-N2 selectivities and high capacities to adsorb CO2 rapidly.Energy Environ. Sci., 5:76647673, 2012. 60http://journals.aps.org/prb/abstract/10.1103/PhysRevB.54.1703http://scitation.aip.org/content/aip/journal/jcp/127/11/10.1063/1.2770708http://scitation.aip.org/content/aip/journal/jcp/127/11/10.1063/1.2770708http://journals.aps.org/prl/abstract/10.1103/PhysRevLett.77.3865http://journals.aps.org/prl/abstract/10.1103/PhysRevLett.77.3865http://journals.aps.org/prl/abstract/10.1103/PhysRevLett.78.1396http://journals.aps.org/prl/abstract/10.1103/PhysRevLett.78.1396http://scitation.aip.org/content/aip/journal/jcp/109/18/10.1063/1.477419http://www.sciencedirect.com/science/article/pii/S0009261489873142http://www.sciencedirect.com/science/article/pii/S0009261489873142http://pubs.acs.org/doi/abs/10.1021/ja309274yhttp://pubs.acs.org/doi/abs/10.1021/ja309274yhttp://www.tandfonline.com/doi/abs/10.1080/01442350050020879http://www.tandfonline.com/doi/abs/10.1080/01442350050020879http://onlinelibrary.wiley.com/doi/10.1002/ceat.200407094/abstracthttp://onlinelibrary.wiley.com/doi/10.1002/ceat.200407094/abstracthttp://pubs.rsc.org/EN/content/articlelanding/2012/cp/c2cp41147dhttp://pubs.rsc.org/EN/content/articlelanding/2012/cp/c2cp41147dhttp://link.springer.com/chapter/10.1007%2F978-1-4020-5295-8_1http://juser.fz-juelich.de/record/3737/files/nic-series-volume42.pdfhttp://www.sciencedirect.com/science/article/pii/S001046551400151910.1016/j.cpc.2014.04.017http://www.sciencedirect.com/science/article/pii/S001046551400151910.1016/j.cpc.2014.04.017http://pubs.acs.org/doi/abs/10.1021/ja01604a001http://pubs.acs.org/doi/abs/10.1021/ja01604a001http://pubs.acs.org/doi/abs/10.1021/jp4048133http://pubs.acs.org/doi/abs/10.1021/jp4048133http://pubs.rsc.org/en/Content/ArticleLanding/2014/CP/C3CP52821Ahttp://pubs.rsc.org/en/Content/ArticleLanding/2014/CP/C3CP52821Ahttp://www.sciencedirect.com/science/article/pii/S0306261913000263http://www.sciencedirect.com/science/article/pii/S0306261913000263http://pubs.rsc.org/en/Content/ArticleLanding/2012/EE/c2ee21153jhttp://pubs.rsc.org/en/Content/ArticleLanding/2012/EE/c2ee21153j[87] D. M. RUTHVEN. Diffusion in type A zeolites: New insights from old data. Microporous Meso-porous Mater., 162:6979, 2012. 61[88] Q. LIU, O. N. C. CHEUNG, A. E. GARCIA-BENNETT, AND N. HEDIN. Aluminophosphates forCO2 separations. ChemSusChem, 4:9197, 2011. 66[89] O. CHEUNG, Q. LIU, Z. BACSIK, AND N. HEDIN. Silicoaluminophosphates as CO2 sorbents.Microporous Mesoporous Mater., 156:9096, 2012. 66[90] O. CHEUNG, Z. BACSIK, P. KROKIDAS, A. MACE, A. LAAKSONEN, AND N. HEDIN. K+ Ex-changed Zeolite ZK-4 as a Highly Selective Sorbent for CO2. Langmuir, 30:96829690, 2014.66http://www.sciencedirect.com/science/article/pii/S1387181111006238http://onlinelibrary.wiley.com/doi/10.1002/cssc.201000256/abstracthttp://onlinelibrary.wiley.com/doi/10.1002/cssc.201000256/abstracthttp://www.sciencedirect.com/science/article/pii/S1387181112000625http://pubs.acs.org/doi/abs/10.1021/la502897phttp://pubs.acs.org/doi/abs/10.1021/la502897pAbstractList of PapersAbbreviations1 Introduction1.1 Background1.2 Zeolites as molecular sieves1.3 Molecular multiscale modeling2 Diffusionally enhanced CO2-over-N2 selectivity in Zeolite NaKA2.1 Zeolite A2.2 Kinetic molecular sieving2.3 Fine-tuning the effective pore window in Zeolite NaKA3 Predicting the CO2 uptake using force field based modeling3.1 Force fields3.2 Modeling the thermodynamic effect with Grand Canonical Monte Carlo3.3 Modeling the kinetic effect with Molecular Dynamics3.4 Predicting the total uptake in narrow pore zeolites4 Predicting the free energy barriers of diffusion using constrained AIMD modeling4.1 Density Functional Theory4.2 Periodic DFT-simulations with CP2K4.3 Constrained AIMD4.4 Determining the free energy barriers of diffusion in Zeolite NaKA4.5 Identifying the local diffusion rate-determining properties5 Scaling up: Coarse graining the time evolution with Kinetic Monte Carlo5.1 Kinetic Monte Carlo5.2 Determining the rate constants5.3 KMC-simulations with KMCLib5.4 Modeling the CO2 and N2 uptake in a realistic Zeolite NaKA powder particle model5.5 Testing the effects of rate-determining properties5.6 Adsorption kinetics6 Conclusions and OutlookSammanfattning p svenskaAcknowledgementsReferences